* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

High-temperature superconductivity wikipedia, lookup

Photon polarization wikipedia, lookup

Introduction to gauge theory wikipedia, lookup

Electromagnetism wikipedia, lookup

Superconductivity wikipedia, lookup

State of matter wikipedia, lookup

Hydrogen atom wikipedia, lookup

Nuclear physics wikipedia, lookup

Electrical resistivity and conductivity wikipedia, lookup

Nuclear structure wikipedia, lookup

Theoretical and experimental justification for the Schrödinger equation wikipedia, lookup

Condensed matter physics wikipedia, lookup

Density of states wikipedia, lookup

Transcript

Theoretical Investigations on Mixedvalence Transition-metal Oxides by RAVINDRAN VIDYA Dissertation presented for the degree of Doctor Scientiarum 2005 Department of Physics Faculty of Mathematics and Natural Sciences University of Oslo Norway To my Family What we have learned is a handful of sand. What we have yet to learn is the whole world. - Tamil poetess Avvaiyar (ca. 200 B.C.) Preface If I have been able to see farther than others it is because I stood on the shoulders of giants. Sir Isaac Newton I am truly honored to submit my thesis for the degree of Dr. Scient. at the Department of Physics, Faculty of Mathematics and Natural Sciences, University of Oslo. This thesis is a fruit of four years of dedicated research. It would not have been made possible or had not taken the shape it has now, without the help and support of many people. I feel this is the right time and place to pay my tribute for these contributions. First of all, I wish to express my sincere thanks to Prof. Leif Veseth for accepting me as his Ph.D student. Even though I have registered my doctor project at the Department of Physics, the actual research work has been carried out at the Department of Chemistry under the daily guidance of Prof. Helmer Fjellvåg, Prof. Arne Kjekshus, and Dr. P. Ravindran. I render my sincere gratitude to Helmer for his many insightful discussions, showing keen interest in my works, and providing me the necessary infrastructure facilities. I am most indebted to Arne for many scientific discussions (especially enlightening me on magnetism among many other subjects), his skilful guidance, and caring enquiries on the progress of the project. I am ever grateful to Arne for being patient and devoting his valuable time in improving the quality of the manuscripts (in fact, toward the end I flooded him with too many manuscripts in too short a time). I am truly privileged to sit beside a living “encyclopedia", Dr. P. Ravindran who formulated the main-stream project, giving new ideas and directions to move ahead in addition to providing computational tools from his treasury. The letter “P" in his name must certainly stand for perseverance, who taught me that perseverance and determination are most important in life. I kindly acknowledge him for actively participating in discussions and continuously motivating me to use different tools to bring out the real truth and thereby understand the underlying physics. I also extend my warm thanks to Dr. P. Vajeeston for fruitful colloboration and many helps with the PC. I wish to gratefully acknowledge Professors O.K Anderson, O. Jepsen, J.M. Wills, and O. Eriksson, for allowing me to use their computational codes. I wish to thank Prof. P. Blaha, Prof. G. Kresse, Prof. Bjørn Hauback, Dr. Pavel Korzhavyi, Dr. Karel Knizek, Dr. Smagul Zh. Karazhanov, Dr. Anna Delin, Dr. Alexei Grechnev, Laila Offernes, Ole Bjørn Karlsen, and Arne Klaveness for useful communications. I kindly acknowledge the Research Council of Norway (NFR) and the Department of Physics for providing me the financial support. The project has been successfully carried out using the Norwegian Supercomputer facilities (NOTUR). I express sincere thanks to NFR for providing the supercomputer time and the staff at NOTUR consortium for their support. I also acknowledge the computer supports provided by our friends at local [email protected] and USIT. I take this opportunity to thank all my friends in “Seksjon A" for providing a pleasant working environment. ext my greatest gratitude goes to my parents and brother who are always there to share my pleasure and pain. I should admit that without their constant support and encouragement, this could not have been made possible. I extend my warm thanks to all my relatives and friends (here in Oslo and elsewhere) who through their loving calls from miles away enquired my progress and encouraged me. I also take this opportunity to thank all my school, college, and university teachers who have sown in me a keen interest for science which actually has taken me thus far in life. Last but certainly not the least, I am ever grateful to my husband Ravi for his patience and understanding. I wish to appreciate the love of my two year old son Vighnesh, who with his pure innocent smiles refreshes my mind and recharges my brain. I owe a lot to both of you. I thank one and all and wish the readers a happy reading. N University of Oslo, November 2005 Vidya CONTENTS Preface 5 Part I 7 1 2 3 Introduction 1.1 Materials Science . . . . . . . . . . . . . . 1.2 Computational Materials Science . . . . . 1.2.1 Density-functional theory . . . . . 1.3 Thesis outline . . . . . . . . . . . . . . . . 1.3.1 Spin, charge, and orbital Ordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 11 12 13 14 14 Theoretical Background − Many-body Problem 2.1 The Hartree approximation . . . . . . . . . . 2.2 Hartree−Fock approximation . . . . . . . . . 2.3 Density-functional theory (DFT) . . . . . . . 2.3.1 Theorem 1 . . . . . . . . . . . . . . . . 2.3.2 Theorem 2 . . . . . . . . . . . . . . . . 2.4 Spin-polarized systems . . . . . . . . . . . . . 2.4.1 Exchange-correlation energy . . . . . 2.4.2 Generalized-gradient approximation 2.5 Limitations of density-functional theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 18 19 20 20 20 21 22 23 24 Computational Techniques 3.1 Periodicity and crystal symmetry 3.2 Electronic structure methods . . 3.3 The LMTO method . . . . . . . . 3.3.1 Muffin-tin orbitals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27 28 29 30 30 . . . . . . . . 7 . . . . . . . . . . . . . . . . . . . . . . . . . CONTENTS . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 32 33 34 35 36 37 38 39 41 42 43 44 44 44 Ground-state Properties and their Analyses 4.1 Structural stability and Phase transitions . . . . . . . . . . . . 4.2 Electronic Structure . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 Classification of materials . . . . . . . . . . . . . . . . 4.2.2 Density of states . . . . . . . . . . . . . . . . . . . . . 4.3 Bonding Characteristics . . . . . . . . . . . . . . . . . . . . . 4.3.1 Types of bonding . . . . . . . . . . . . . . . . . . . . . 4.3.2 Partial density of states . . . . . . . . . . . . . . . . . 4.3.3 Crystal-orbital-Hamiltonian-population (COHP) plot 4.3.4 Charge-density plot . . . . . . . . . . . . . . . . . . . 4.3.5 Charge-transfer plot . . . . . . . . . . . . . . . . . . . 4.3.6 Electron-localization function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47 47 48 48 49 50 51 52 54 55 55 57 Excited-state Properties 5.1 Excitations in Density-Functional Theory . . . . . . . . 5.2 Definition of the Conductivity Tensor . . . . . . . . . . 5.2.1 Symmetry considerations . . . . . . . . . . . . . 5.2.2 Broadening . . . . . . . . . . . . . . . . . . . . . 5.2.3 Indirect interband and intraband contributions . 5.3 Extracts of theory of optics . . . . . . . . . . . . . . . . . 5.3.1 Index of refraction . . . . . . . . . . . . . . . . . 5.3.2 Reflectivity . . . . . . . . . . . . . . . . . . . . . 5.3.3 Absorption coefficient . . . . . . . . . . . . . . . 5.3.4 Energy loss . . . . . . . . . . . . . . . . . . . . . 5.4 A note on spin-orbit coupling . . . . . . . . . . . . . . . 5.5 Calculation of Magneto-Optical Properties . . . . . . . 5.5.1 Magneto-optical figure-of-merit . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 59 59 60 61 63 63 64 65 65 65 66 66 66 68 3.5 3.6 3.7 3.8 4 5 3.3.2 The LMTO − atomic sphere approximation method Full potential methods . . . . . . . . . . . . . . . . . . . . . 3.4.1 The full potential LMTO method . . . . . . . . . . . 3.4.2 The basis set . . . . . . . . . . . . . . . . . . . . . . . 3.4.3 The LMTO matrix . . . . . . . . . . . . . . . . . . . Full potential LAPW method . . . . . . . . . . . . . . . . . 3.5.1 The LAPW basis and its properties . . . . . . . . . . Pseudopotential Method . . . . . . . . . . . . . . . . . . . . The projected augmented wave (PAW) method . . . . . . . 3.7.1 Charge density . . . . . . . . . . . . . . . . . . . . . 3.7.2 Total energy . . . . . . . . . . . . . . . . . . . . . . . Brillouin zone integration . . . . . . . . . . . . . . . . . . . 3.8.1 Special points method . . . . . . . . . . . . . . . . . 3.8.2 Tetrahedron method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4 8 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . CONTENTS 5.6 6 7 8 Calculation of XANES . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Magnetism and Spin Ordering 6.1 Magnetic classes . . . . . . . . . . . . . . . 6.2 Types of antiferromagnetic spin ordering 6.3 Exchange interaction . . . . . . . . . . . . 6.3.1 Double-exchange interaction . . . 6.3.2 Super-exchange interaction . . . . 69 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 71 71 74 75 76 77 Charge and Orbital Ordering 7.1 Mixed-valence transition-metal oxides . . . . . . . . . . . . . . . . . 7.1.1 Determination of valence states . . . . . . . . . . . . . . . . . 7.1.2 Effects of crystal-field . . . . . . . . . . . . . . . . . . . . . . 7.2 Influence of structure on ordering phenomena . . . . . . . . . . . . 7.2.1 Effects of Jahn-Teller distortion . . . . . . . . . . . . . . . . . 7.3 Orbital Ordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.1 An example−LaMnO3 . . . . . . . . . . . . . . . . . . . . . . 7.4 Charge ordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.1 Types of charge and orbital ordering . . . . . . . . . . . . . . 7.5 Charge and orbital ordering in oxygen-deficient double perovskites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 79 79 80 81 81 83 84 84 85 86 88 Summing Up and Looking Ahead 8.1 Scientific highlights . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 General Inferences . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3 Next step . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 91 92 95 96 Bibliography . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 97 Part II 103 List of publications 105 Appendix 107 9 CONTENTS 10 CHAPTER 1 Introduction Knowledge advances by steps and not by leaps. Lord Macaulay 1.1 Materials Science An important and widely acclaimed feature of materials science has been the recognition of the fundamental similarities underlying the structures, phenomena, and properties of a wide variety of interesting and technologically important materials. This has led to an unusually large degree of cross-fertilization of ideas and approaches among several different traditional scientific and engineering fields. Not only all properties and qualities of matter but also all fields of human concern are involved in the interaction between the macro- and microscopic levels of the atomic architecture. To the age-old question: “which comes first, the chicken or the egg?", a probable response of a materials scientist would be: “neither”. In material science there is a synergism between what exists and what needs to exist. Materials are mostly designed with a particular application in mind.1 Owing to the capacity of man for immediate aesthetic interaction with materials, quite subtle materials were discovered very early. It began simply with the collection of beautiful natural objects and the discovery that heating and mixing changed their qualities to yield materials that could be used for more than “mere” enjoyment. This aesthetic involvement spurred continual search, and quite advanced materials technology were developed long before mechanical technology. Until about 1800 AD knowledge of materials and the practical control of their composition and properties to achieve a desired result were more advanced in the Far Eastern than in Western cultures [1]. One may venture a guess that this was because Eastern culture put slightly greater emphasis upon an aesthetic approach to the 1 Indeed some new materials, such as nylon, the first polymer, were discovered simply by chance. CHAPTER 1. INTRODUCTION world rather than a logical advance. It has long been recognized that ingenious developments of materials coincide with important stages in the development of civilizations. The current efflorescence of materials science and engineering is certainly coincident with great social changes. Materials were handled in accordance with their nature that has been learned sensitively, but theoretical understanding of the reasons for their properties developed slowly and had little or no effect on the practice until the last century [1]. For a long period of time structure-sensitive properties other than magnetism were invisible to physicists, and it was mainly practical artisans and a few more theoretically inclined chemists and metallurgists who kept alive knowledge of real solids and slowly accumulated facts that eventually forced the birth of the new physics of solids. 1.2 Computational Materials Science Medieval alchemists dreamed of transmuting common base metals into gold, but such miraculous conversions proved impossible, of course. One of the most promising developments in materials research − computational materials science − is sometimes referred as “computational alchemy” Today, thanks to discoveries in the fields of computational physics and computational chemistry, researchers are making startling progress in understanding and manipulating matter at the atomic and molecular level. This has been fueled by the increasing performance of state-of-the-art supercomputers and high performance workstations. Researchers in this field have acquired enough confidence in their arsenal of computational methods in order to make bold predictions that have run ahead of experiments or in some cases, even corrected them. The opportunities for computational research are as broad as they are deep. All kinds of materials are dealt with, without any restriction. Ultimately, we hope that new understanding of all of these materials will be transferred to making new materials with properties that mankind can use. Because of the detailed perspective they offer into the behavior of atoms and electrons, we can often significantly enhance and deepen our understanding of how materials function. This approach of using only knowledge of the composition of a material to predict properties is often referred to as first-principles or ab-initio calculation. An obvious advantage of successful first-principles methods is that, since no experimental input is needed, the behavior of a material can be predicted even before it is synthesized. With the increasing capabilities of first-principles methods, some researchers have started to think about computer-based design of new materials. In principle, this should be possible, because all the properties of a material are determined by the constituent atoms and the basic laws of physics. Hence, when material scientists attempt to design new materials, they can quickly focus on promising systems. Moreover, computational experiments have the advantage over real experiments that one has full control over almost all the experimental variables. This level of control makes it possible to design experiments that are optimized to understand the influence of a specific 12 1.2. COMPUTATIONAL MATERIALS SCIENCE variable. As these calculations are not limited to physically realizable states of a material, they can be used to conduct “what-if” experiments. In a calculation it is reasonably simple to change the crystal structure, move or substitute an atom, change the applied pressure, make arbitrary deformations, and so forth, and then to evaluate the effect of these modifications on the properties of interest. 1.2.1 Density-functional theory Since the beginning of quantum mechanics in the 1920’s, one of the most spectacular advances in physics is perhaps the formulation of the density-functional theory (DFT) which enables one to handle many-electron systems with ease. It was constructed by Hohenberg and Kohn [2] in the 1960’s, for which Kohn was awarded the Nobel Prize in chemistry 1998. Since its introduction DFT has evolved into a powerful tool that is widely used in condensed matter theory and computational materials science for the calculation of electronic, magnetic, and structural properties of solids. First-principles simulations using DFT have proved to be a reliable and computationally tractable tool in condensed matter physics. These simulations have now impacted virtually every area of this broad field. Along with the advances in computing technology that have occurred during the last decade, there have been important algorithmic improvements, and for certain classes of materials it is now feasible to simulate systems containing 100 or more atoms in a unit cell. This opens the door for the direct application of these techniques to study a substantial amount of real materials problems. This method has been remarkably successful in reproducing, explaining, and in some cases predicting a wide variety of materials phenomena. Specific examples range from early predictions of phase transitions in silicon under pressure [3] to determination of stable and metastable adsorption geometries on metal surfaces [4], as well as many successes in understanding magnetic materials. The fundamental concept of DFT is that all the ground-state properties of a material are completely determined by the electron charge density ρ(r) − the real space distribution of electrons around the atoms. The contribution of DFT to the science of multi-particle quantum systems (such as molecules and condensed matter) is two-fold. The first contribution is one of understanding; since the inception of quantum mechanics theoreticians were used to think in terms of single-particle orbitals, but when high accuracy is required, the number of Slater determinants increases so much that the comprehension becomes difficult. However, the approach of DFT is different, it focusses on the real three-dimensional space using the electron density ρ(r), a tangible and easily understood entity. The second contribution of DFT is of practical nature. In the conventional quantum mechanics, the handling of systems with many particles (N more than 10-20) becomes cumbersome, since the number of Slater determinants are intractable and hence impossible to handle in practical calculations. As DFT uses ρ(r), it allows for handling of fairly large systems (N ≈ 100−1000), with computational efforts that rise much more moderately with the increasing number of atoms. 13 CHAPTER 1. INTRODUCTION 1.3 Thesis outline The scientific world is broadly divided into basic (or fundamental) research and applied research. For materials scientists involved in basic research, the goal is most often to determine why certain kinds of materials have a particular set of properties. Sometimes predictions of materials properties are made even before the materials themselves are synthesized. On the other hand, applied research involves fashioning materials for real-life applications. It involves knowledge about the conditions under which a material will be used and identifying candidate materials for this purpose. There is always a real need for better materials − the issue is how much better they have to be and at what cost. An applied scientist, with a particular application in mind, will scour lists of known materials looking for one that meets the expected needs. If existing materials are unsuitable, the applied and basic scientist must work together to develop new materials. This synergism between what is available and what needs to be developed reflects the important and complementary roles of the basic and applied sciences in the materials field. This thesis is intended to appeal to both fundamental and applied researchers. The problems have been carefully selected so that, our computational efforts will attempt to answer some of the most fundamental questions relating to technologically-significant materials. Exploring their properties is expected to lead to more understanding and hence to new materials. We believe that with a fundamental understanding at the electronic level of a system comes, a basic scientific appeal and a more complete control over the properties and mechanisms governing any system. This understanding gives the power of prediction which is perhaps the ultimate goal of all sciences. The thesis presented here deals with theoretical calculations of properties like phase stability, electronic structure, magnetic properties, ordering phenomena such as spin, charge, and orbital ordering, and excited-state properties for perovskite-like and complex oxides. The objective of the study has been of a threefold nature: First, to gain further knowledge on a fundamental scientific level of the properties of matter and how these are governed by the electronic structure. Second, to demonstrate the versatility and increased applicability of theoretical calculations as complement to experiments. Third the last, but not the least, objective has been to answer some of the most intricate questions concerned with mixedvalence oxides. 1.3.1 Spin, charge, and orbital Ordering The past few years have seen a flurry of activities in the study of magnetic materials, which previously had an image of "musty physics laboratories peopled by old codgers with iron filings under their fingernails" [5]. In particular, advances in atomic- and nanoscale growth and characterization techniques have led to the production of modern magnetic materials that reveal a range of fascinating phenomena. These phenomena derive from the fact that electrons have spin as well as charge, giving an extra level of complexity to the physics and an extra degree of freedom in device design. Today, the science and technology 14 1.3. THESIS OUTLINE of magnetism have undergone a renaissance, driven both by the urge to understand the new physics, and by demand from industry for better materials. The potential impact on society of the recent advances in magnetic materials is extensive and evidenced by the dramatic enhancement in data-storage density. The discoveries of colossal magnetoresistance (CMR) or [giant magnetoresistance (GMR)] materials, in which magnetic fields cause orders of magnitude changes in conductivity have been particularly significant. Sensors, read heads, and memories based on GMR are already commercially available in the market. In addition to the salient property of magnetoresistance, the CMR (GMR) materials also possess exotic properties such as charge and orbital ordering. Charge ordering is the ordering of valence electrons in a particular fashion below a characteristic transition temperature (Tco ). In the canonical picture of magnetic insulators known since the 1950’s, the electrons occupy fixed atomic orbitals, and the magnitude and sign of the magnetic interaction between neighboring electron spins depend on the relative orientation of the orbitals in which the spin density resides. Orbital order (the fixed pattern of orbital occupations at every atomic site) is usually either built into the crystal structure or changes only at temperatures much exceeding the magnetic ordering temperature (T C ). One of the main objectives of this project has been to gain understanding of such ordering phenomena. The basic requirement for charge ordering to take place is the presence of an element (usually a transition-metal constituent) in different valence states. Even though a lot of attention has been paid to mixed-valence manganese oxides, it should be noted that the orbital physics is universal in transition-metal oxides. Hence we have attempted to analyze compounds (particularly perovskite-like and complex oxides) containing mixed-valence transition-metal constituents such as Cr, Mn, Fe, and Co. We believe that a basic understanding of mixed valence and hence charge and orbital ordering will provide new understanding and in turn new materials. The thesis has been disposed of as three main segments. The first part should appeal to readers with a general background and broad-line interests. The second part deals with introductions to the theoretical background and the topics covered in the present project. The third part is more detailed and intended to give a thorough analysis of the results obtained from the theoretical studies. This part is further complemented by direct access to the articles and publications themselves together with relevant references. In all segments, the aim is to spark the basic curiosity of the readers and make them dwell deeper with the science. 15 CHAPTER 1. INTRODUCTION 16 CHAPTER 2 Theoretical Background − Many-body Problem Make things as simple as possible, but not simpler. Albert Einstein C ondensed matter physics and materials science are concerned with the fundamental understanding and exploitation of properties of systems with interacting electrons and atomic nuclei. The electrons and nuclei that compose a given material constitute a strongly interacting many-body system. The properties of matter are governed by the behavior of the almost mass-less electrons that move around the much heavier nuclei. This has been well known since the early days of quantum mechanics. With this comes the recognition that, at least in principle, almost all properties of materials can be addressed given suitable computational tools. In order to describe real matter, we need to device theoretical tools that are capable of dealing with the interactions between a very large number of particles, typically of the order of moles, i.e., 10 23 particles; which is a Herculean task to exploit indeed. Hence we need to resort to approximations and simplifications. The Schrödinger equation is the basic tool to study the properties of a given material. The time-independent Schrödinger equation has the operator form [6] (2.1) Hψ = Eψ where H is the Hamiltonian operator, E is energy, and ψ is the wave function. Eq. 2.1 can be exactly solved in the case of one nucleus and one electron, viz. for hydrogen and hydrogenlike systems. However, a more realistic situation comprises a many-particle wave function ψ(r1 , r2 , ..ri , ..rN ), where ri denotes the position of particle i. The 10 23 ingredients of a typical solid make the problem complicated. The Hamiltonian for the whole bulk system is H=− h̄2 2 1 1 Zk Zl e2 Zk h̄ ∇2 − − . + ∇i + 2 Mk 2 |Rk − Rl | 2m 2 |ri − rj | |ri − Rk | k k=l i i=j i,k (2.2) CHAPTER 2. THEORETICAL BACKGROUND − MANY-BODY PROBLEM In this Hamiltonian h̄ (= h/2π, h is the Planck constant), m and rk denote the electron mass and the respective coordinates, M k and Rk nuclear masses and the respective coordinates, and Z is the charge of the constituent nuclei. The indices i and j number the electrons and k and l the nuclei. The first term in Eq. 2.2 denotes the kinetic energy of the nuclei, the second term the Coulomb energy between the nuclei, the third term the kinetic energy of the electrons, the fourth term the interaction among the electrons, and the last term denotes the electrostatic interaction between the electrons and the nuclei [which can be regarded as an external potential (Vext ) acting upon the electrons]. The motions of the nuclei, notably originating from lattice vibrations, in most materials is on a much larger time scale than typical electronic scale, so that the electrons may be considered to be in their instantaneous ground state as the nuclei move. Hence, in this so-called "Born-Oppenheimer" approximation, the nuclei are considered to be stationary, and Eq. 2.2 has to be solved for the electrons around these stationary nuclei. This allows us to remove the first term in Eq. 2.2. The second term is only a constant (since the nuclear positions are known), and is not to be considered until we actually calculate the total energy. Now, the total energy Hamiltonian can be expressed as H=− i ∇2i + 2Zk 1 − . |ri − rj | |ri − Rk | i=j (2.3) i,k Here we have also introduced the Rydberg atomic units, i.e., e 2 = 2, h̄ = 1, and m = 12 . In order to solve the Schrödinger equation for all the interacting electrons, we have to solve a system of around 1023 simultaneous differential equations. Such a calculation is beyond the capabilities of present-day computers, and is likely to remain so for the foreseeable future. 2.1 The Hartree approximation The Hartree approximation provides a way to simplify Eq. 2.2 so that it can be solved somewhat easily. In Eq. 2.2, the potential experienced by an electron depends on the positions of the other electrons. However, this potential can be approximated by an average single-particle potential called the Hartree potential which is not coupled to the individual motions of all the other electrons, but depends simply upon the time-averaged electron distribution of the system. It is given by Vd (ri ) = e2 j=i nj |ψj (rj )|2 , |ri − rj | (2.4) where nj are the orbital occupation numbers and ψj (rj ) is a single-particle wave function, i.e., a solution to the one-particle wave-equation: − h̄2 2 ∇ + Vext + Vd (ri ) ψi (ri ) = εi ψi (ri ) 2m 18 (2.5) 2.2. HARTREE−FOCK APPROXIMATION Thus, the set of equations now becomes separable. However, the equations are still non-linear and have to be solved self consistently by iteration. Even though the Hartree approximation allows one to calculate the approximate single-particle wavefunctions for the electrons in solids, it has a few drawbacks. According to the Pauli-exclusion principle, two electrons can not exist at the same point in space with the same set of quantum numbers. However, the wave function in Hartree theory Ψ(r1 σ1 , r2 σ2 , ..., rN σN ) = N ψi (ri , σi ) (2.6) i is not antisymmetric for interchange of electron coordinates and accordingly does not follow the Pauli-exclusion principle. Moreover, the Hartree approximation fails to describe how an electron is affected by the configuration of the N −1 other electrons. These defects have been rectified by the Hartree−Fock theory. 2.2 Hartree−Fock approximation Already in 1930 Fock pointed out that, any approximation to the true wave function should explicitly include spin and should be antisymmetric to interchange of electrons. Hence, instead of the "simple" spatial orbitals, one must use spin orbitals and moreover take into account antisymmetric linear combinations of products of spin orbitals. We assert that a solution of Eq. 1 is given by any state Ψ that makes the following quantity stationary: (Ψ, HΨ) (2.7) Ψ, Ψ According to the variational principle [7], the normalized expectation value of energy is minimized by the ground-state wave function Ψ. A better description is to replace the wave function in Eq. 2.6 by a Slater determinant of one-electron wave functions Ψ1 (r1 σ1 ) Ψ1 (r2 σ2 ) . . . Ψ1 (rN σN ) Ψ2 (r2 σ2 ) . . . Ψ2 (rN σN ) 1 Ψ2 (r2 σ2 ) (2.8) Ψ(r1 σ1 , r2 σ2 , . . . , rN σN ) = √ . . .. .. .. .. . N ! . . ΨN (rN σN ) ΨN (rN σN ) . . . ΨN (rN σN ) E= This is a linear combination of products of the form given by Eq. 2.6 and all corresponding products are obtained by permutation of r i σi among themselves. The Hartree−Fock equation which follows from energy-minimization is given by: e2 h̄2 2 ∇ + Vext + Vd (ri ) ψi (ri ) − ψ (r )ψi (r )ψj (r)δsi sj = εi ψi (ri ) d − 2m |r − r | j j 19 (2.9) CHAPTER 2. THEORETICAL BACKGROUND − MANY-BODY PROBLEM Hence, in addition to the Hartree potential, another potential called the exchange potential (the last term on the left hand side of Eq. 2.9) operates only between electrons with the same spin. In addition, there should also be a correlation interaction (resulting from simple electrostatic interaction between the electrons), which is not included here. Consequently, the correlation energy can be described as the difference between the exact energy for the system and the Hartree−Fock energy. 2.3 Density-functional theory (DFT) Since the ground-state electronic structure is the most important quantity in determining the material properties, we need a robust and very accurate method to describe the electronic structure. It is well known that the properties of matter are governed by the electrons surrounding the atomic nuclei and interactions between them. Hence, if one could get hold of the real space distribution of these electrons [viz. the electron charge density ρ(r)] then almost all physical properties can be predicted. The objective of the electronic structure calculations is to obtain the electron density. The most important milestone of modern day quantum mechanics is the development of DFT [8]. By far, the most accurate "first-principles" quantitative calculation of ρ(r) is based on DFT which is able to distinguish small energy differences between very different phases of a given material. DFT is so successful that it has now become one of the most widely used modern theories to understand the properties of matter. Hohenberg and Kohn suggested in 1964 that the many-electron wavefunction is a too complicated entity to deal with as a fundamental variable in a variational approach. Hence, in their density-functional formalism which is based on two theorems first introduced by Hohenberg and Kohn [2] and later extended by Kohn and Sham [9], they suggested a different quantity. 2.3.1 Theorem 1 For an interacting system of electrons in an external potential, V ext (r), there exists a universal functional of the charge density, F [ρ(r)], independent of V ext (r), that provides the electronic energy: E= Vext (r)ρ(r)dr + F [ρ(r)]. (2.10) 2.3.2 Theorem 2 The functional F [ρ(r)] obtains its minimum value (viz. the ground-state energy) for the actual electron-charge density of the system [2]. The electron-charge density can be obtained from the solution of an associated singleparticle problem, whose effective single-particle potential Vef f [r, ρ(r)], is the sum of the external potential, and a unique functional of ρ as given below. As a consequence, the calcu20 2.4. SPIN-POLARIZED SYSTEMS lation of the energy in terms of ρ(r) is reduced to the self-consistent solution of a system of coupled, non-linear, one-electron-like Schrödinger equations: 1 2 ρ(r ) δExc [ρ] − ∇ + Vext (r) + dr + φi (r) = i φi (r), (2.11) 2 |r − r | δρ( r) The so-called Kohn-Sham (KS) wavefunctions, φi , are single-particle eigenfunctions that are strictly meaningful only for determining ρ(r). The KS eigenvalue i , which is the derivative of the total energy with respect to the occupation of state i, is used in determining which one-electron states are occupied: states are filled from the lower eigenvalues to the higher, without regard to the spin parameter. The eigenvalues are not strictly related to single-particle excitation energies, although further theoretical considerations can explain why KS-band structures become a useful tool in the interpretation of spectroscopic (especially photoemission) data. For an arbitrary electron-charge density there is no simple explicit expression for the exchange correlation energy E xc . The widely used local-density approximation (LDA) is a simple approach, exact within the limit of a homogeneous electron density, and leads to remarkably accurate results for many classes of materials. Within the LDA, Exc is written as (2.12) Exc (ρ) = ρ(r)Exc [ρ(r)]dr, where Exc (ρ) is the exchange-correlation energy of a uniform interacting electron gas of density ρ. The use of LDA is strictly speaking, justified only if ρ(r) is a slowly varying function, and a number of extensions exist which give improved accuracy for systems with more localized electrons. 2.4 Spin-polarized systems In the generalization of DFT to spin-polarized systems, the charge density ρ(r) is decomposed into the two spin densities (ρ ↑ and ρ↓ ) as ρ(r) = ρ↑ (r) + ρ↓ (r) (2.13) The Hohenberg-Kohn theorem in this case postulates that the ground-state total energy is a functional of the spin densities. (2.14) E = E[ρ↑ , ρ↓ ] The total energy consists of terms like those for the non-spin-polarized case. The Coulomb terms remain functionals of the total energy, but E s (viz. single-particle kinetic energy) and Exc become functionals of the two spin densities. There are separate sets of KS orbitals for the two spin components, and two sets of single-particle equations need to be solved to obtain them. The variational principle is invoked to generate the spin-polarized KS equations of spin-density-functional theory. (T + Vei (r) + VH (r))φiσ (r) = iα φiσ (r) 21 (2.15) CHAPTER 2. THEORETICAL BACKGROUND − MANY-BODY PROBLEM where σ is the spin index and the density is given by a sum over the occupied orbitals. ρσ (r) = φiσ (r)φiσ (r) (2.16) occ and the highest occupied orbital is determined by the electron count. V xc is the only term in the single-particle Hamiltonian that is explicitly spin dependent. Vxc,σ = δExc [ρ↑ , ρ↓ ] δρσ (r) The total-energy expression then becomes, 1 d3 rVH (r)ρ(r) − d3 r(ρ↑ (r)Vxc,↑ (r) + ρ↓ (r)Vxc,↓ ) + Exc [ρ↑ , ρ↓ ] − E = Eii + 2 occ (2.17) (2.18) These equations are to be solved self-consistently as in the non-spin-polarized case. In the above expression, Eii is the electron-electron interaction energy and E xc is a functional of the two spin densities. E xc favors spin-polarized solutions and Ts opposes such an outcome. A balance between these two terms determines whether a material is magnetic or not (neglecting diamagnetism). Because of the additional degrees of freedom contained in the spin-density case, spinpolarized KS equations often have multiple self-consistent solutions, corresponding to different stable spin configurations. Hence, in order to determine the real ground state (corresponding to the lowest energy), all possible spin configurations should be considered in the calculations. Moreover, the dimension of the matrix corresponding to the Hamiltonian operator for a magnetic system will be twice the dimension of the matrix representing the non-magnetic system. The upper left quarter of the matrix represents one spin channel and the lower right quarter of the matrix represents the other spin channel. The off-diagonal elements correspond to hybridization between different spins and/or rotated spin coordinates. 2.4.1 Exchange-correlation energy The exchange potential for a system of variable density can be approximated by a term [ρ(r)]1/3 , where ρ(r) represents the local density. This [ρ(r)] 1/3 dependence is a consequence of the exchange (Fermi) hole. The Fermi hole is a region surrounding each electron in which the probability of finding another electron with the same spin is small. In other words, this hole is the region near an electron which is avoided by electrons with the same spin. Modern DFT approximates the full non-local exchange with a term based on the local density, hence called the local density approximation (LDA). The exchange-correlation term is to some extent approximated in the current theoretical framework. Since the electrons interact with each other, they correlate their motion so that they tend to avoid each other. The correlation (Coulomb) hole is the region surrounding each electron in an atom in which the probability of finding another electron is small. An electron at r reduces the probability 22 2.4. SPIN-POLARIZED SYSTEMS of finding another electron at a nearby position r , and every electron is surrounded by a hole in the electron density of equal and opposite charge [10]. In the local spin density approximation (LSDA) the exchange-correlation energy is written as LDA (2.19) Exc = drρ(r)xc [ρ↑ (r), ρ↓ (r)], where xc is the exchange-correlation energy per particle in a homogeneous spin-polarized electron gas. We can also describe an exact term for the exchange-correlation energy using exchange-correlation holes [10]: 1 1 d(r)ρ(r) dr ρxc (r, r − r), (2.20) Exc = 2 |r − r| where ρxc (r, r − r) is the exchange correlation hole which obeys the sum rule (total charge equals to −1): (2.21) dr ρxc (r, r − r) = −1. It can be shown that on making a variable substitution R = r − r, Exc can be written as [10]: ∞ 1 2 1 d(r)ρ(r) dΩρxc (r, R), dRR (2.22) Exc = 2 |R| 0 which in turn implies that the exchange energy depends only on the spherical average of ρxc . Here lies the answer to why the LDA approximation works so well. The point is that even if LDA does not give the right form for the exchange-correlation hole it does give a spherical average which is very close to the real charge distribution [10]. The LDA is widely used in solid state physics, but there are more modern improvements suitable to treat the full non-local exchange such as the generalized gradient approximation (GGA), where Exc has become more composite on introduction of contributions also from the gradient of the local density. 2.4.2 Generalized-gradient approximation One of the promising avenues for refinement of the LDA is the GGA approach. In GGA, the function Exc (ρ) is replaced by a local function of the charge density and the magnitude of its gradient, Exc (ρ, |∇ρ|); the rational is that a better description might result from incorporation of the additional information contained in the local gradient. GGA-based calculations have been reported for a wide variety of materials using several different parameterizations of the GGA functionals. From these calculations it is found: (1) GGAs significantly improve the ground-state properties for the light elements, molecules and solids composed of these, (2) many properties of the 3d transition metals are improved, for example the correct bcc ground state for Fe is obtained, (3) magnetic energies for the 3d transition metals may be 23 CHAPTER 2. THEORETICAL BACKGROUND − MANY-BODY PROBLEM overestimated, and (4) the GGAs lead to excessive increases in the unit-cell parameters for some materials containing heavy elements, and consequently degraded agreement with experiment compared to the LDA [11]. The exchange-correlation energy is given as a (spin) density gradient of the form: GGA Exc [ρ↑ , ρ↓ ] = drf (ρ↑ (r), ρ↓ (r), ∇ρ↑ (r), ∇ρ↓ (r)), (2.23) where the function f is chosen according to certain criteria. Exchange-correlation approximations in the above form are semilocal in the sense that the energy density at r depends on the electron density in an infinitesimal neighborhood of r. There are quite a few GGA functionals available, named after the inventors as Langreth-Mehl, Perdew-Wang 86, BeckePerdew, Lee-Yang-Parr etc. However, in the present project we have used only the PW91 and PBE GGA functionals. Perdew-Wang 91 (PW91) The PW91 [12] approach is similar to LSDA as well as gradient expansion approximation (GEA) but it is purely ab initio. It is constructed using only uniform electron-gas data for exact conditions. PW91 includes a real space cut-off also for the correlation functional and takes the Becke exchange with only small refinements. It fulfills almost all of scaling relations, including those found after the formulation of functional. Perdew-Burke-Ernzerhof (PBE) The PBE [13] approach simplifies the cumbersome derivation of PW91 and corrects some of its minor flaws such as the spurious wiggles in the exchange-correlation potential for small and large (dimensionless) density gradients. However, the resulting energies change only marginally. 2.5 Limitations of density-functional theory Every theory has its own advantages as well as limitations, like two sides of a coin. DFT provides no exception. Fundamentally, DFT only concerns the electronic groundstate structure and underestimates band gaps, which for some semiconductors come out incorrect by 10−30%. A famous (and for this project very relevant) error is also found for transition-metal oxides that are predicted to be metallic, whereas they actually are semiconductors/insulators. Other traditional short-comings of the DFT have been attributed to failures of the specific exchange-correlation functions used, e.g., the failure to predict the bcc ground-state structure of Fe. When GGA is used instead of LDA, the correct groundstate structure is expectedly obtained. In practice, it is a complicated matter to single out the exact reason for the failure in a given calculation, since there are usually an appreciable number of approximations involved. However, it should be stressed that although there 24 2.5. LIMITATIONS OF DENSITY-FUNCTIONAL THEORY are limitations to the applicability of the DFT (along with exchange-correlation functionals), one should not to be too pessimistic. Instead, one should view these procedures as computational exercises and simply try to push the limits of the theory, of course always trying to validate the findings with experimental facts. 25 CHAPTER 2. THEORETICAL BACKGROUND − MANY-BODY PROBLEM 26 CHAPTER 3 Computational Techniques Do not worry about your difficulties in mathematics. I can assure you mine are still greater. Albert Einstein D FT based electronic structure methods are classified according to the representations that are used for the density, potential and, most importantly the Kohn-Sham orbitals. The choice of representation is made to minimize the computational costs of the calculations, while maintaining sufficient accuracy. These competing material- and application-dependent goals have led to the development and use of a wide variety of techniques. In this chapter, we will briefly explain some of the techniques for solving the singleparticle equations for crystalline solids and outline the difference between methods that have been used in this thesis. [−∇2 + Vef f (r)]ψi (r) = εi ψi (r). (3.1) From this equation we can find the electron charge density ρ(r) ρ(r) = N |ψ j |2 . (3.2) j=1 Because both the electrostatic potential (Φ) and V xc depend on ρ(r) we can calculate a new Vef f (r) using the local-density approximation, GGA etc. for the exchange-correlation and the Poisson equation for the electrostatic contribution: ∇ Φ(r)i = −4π 2 N |ψj |2 . (3.3) j=1,j=i We repeat this process until self-consistency is reached [viz. the difference between Vef f (r) in the m and m−1 iterations is less than a predetermined value; the difference being CHAPTER 3. COMPUTATIONAL TECHNIQUES the only chosen convergence criterion]. When self-consistency has been reached, we calculate the total energy of the system of electrons and nuclei using the total-energy expression of the functionals Eq.(2.10) 3.1 Periodicity and crystal symmetry It would have been an impossible task to solve the equations if we had to perform the calculations for all electrons in a given material. The calculations performed by DFT is usually for a unit cell of a crystal. (A crystal is an ordered state of matter in which the positions of the nuclei and consequently all properties are repeated in space.) Fortunately the potential is periodic for an infinite crystal, i.e., invariant under lattice translation T and hence solving the equations in some reduced part of the system will provide the solution for the entire system since the solution will necessarily repeat itself with the translational symmetry of the crystal. V (r + T) = V (r), (3.4) T = m1 a1 + m2 a2 + m3 a3 . (3.5) The vectors {ai } are the real-space Bravais lattice vectors that span the crystal structure and {mi } are integers. According to the Bloch theorem, the eigenstates can be chosen to takes the form of a plane wave times a function with the periodicity of the Bravais lattice; ψk (r + T) = eik.T ψk (r) (3.6) where k is the Bloch wave vector. Now, the one-electron function can be characterized by the Bloch vector k. As a consequence, Eq. (3.1) can be rewritten as Hef f (r)ψn (k; r) = εn (k)ψn (k; r), (3.7) where the index i in Eq. (3.1) has been replaced by the quantum number n. The one-electron wave function ψn and the corresponding eigenvalues ε n are now characterized by the Bloch wave vector k. The phase factor takes the value 1 for some electronic states. This happens when the wave-vector corresponds to a reciprocal lattice vector defined by g = 2π(n1 b1 + n2 b2 + n3 b3 ) (3.8) where ni are integers and bi are the basis vectors of the reciprocal lattice, i.e., (ai .bj ) = δij For k = g 28 (3.9) 3.2. ELECTRONIC STRUCTURE METHODS eik.T = eig.T = e2πimi ni = 1. (3.10) Thus a periodicity in real space also introduces a periodicity in reciprocal space (k), and an electron state with wave vector k = k + g will consequently satisfy the Bloch condition. To describe the electronic structure of a solid it is thus not necessary to consider the vectors, we can consider only the wave vectors contained inside the region of the reciprocal space known as Brillouin zone (BZ). In addition to the translation symmetry, the crystal also obeys symmetries under rotations, implying that there are symmetry operations which transform one wave vector into another wave vector and that reduces our problem further. The smallest possible zone which defines a complete set of symmetry independent wave vectors is called the irreducible part of the BZ. For example, in a simple cubic lattice, the irreducible part of the BZ is only 1/48 of the full BZ and this is the only part we need to find a solution for in such an electronic structure problem. 3.2 Electronic structure methods In order to solve Eq. 3.7 we need to expand it in a basis of known functions, and we have to resort to one of the available electronic structure methods. The choice of basis-functions is crucial for the efficiency of a given computational method and the first step in the implementation of a DFT method is to find a suitable basis set. (1) Basis sets that obey the Bloch condition explicitly, viz. the expansion involves basis functions that are fixed and the coefficients c n are chosen to minimize the energy. ψ(r) = cn φn (r) (3.11) n One disadvantage of this approach is that the wave functions are fixed, which often leads to considerable difficulties in obtaining a sufficiently converged basis set. (2) The other group involves wave functions that can be varied. The variation is promoted by introducing energy-dependent wave functions φ n (ε, r) of the form ψ(ε, r) = cn φn (ε, r), (3.12) n However, the Bloch conditions are no longer automatically fulfilled. The solutions in one unit cell are now chosen to fit smoothly to those of the neighboring cells, thus fulfilling the Bloch condition "indirectly". As the wave function can be modified to the problem at hand, these techniques converge very fast for the number of required basis functions. Every k point of the band structure must be solved for a large number of ε. Solutions only exist when ε are actual eigenvalues. While computation based on these methods are accurate, they are also time consuming. A solution to this problem is to linearize the energy dependent orbital basis. The basis is introduced in the form of a Taylor expansion in ε so that the orbitals themselves are energy independent, although the expansion retains the energy dependence. 29 CHAPTER 3. COMPUTATIONAL TECHNIQUES The variational equation (3.7) thus has to be solved only once for each k point. Such methods are extremely rapid and slightly less accurate than other non-linear methods. 3.3 The LMTO method r Ψ (E,r) l SE 0 SMT 0 SMT S r E (c) (a) V(r) ε κ2 0 VMTZ (b) Figure 3.1: The muffin-tin approximation. (a) the muffin-tin sphere with radius SMT , and the describing sphere of radius SE . (b) the muffin-tin part of the crystal potential V (r), and (c) the radial part of the wave function. During the last decades, the linear-muffin-tin-orbital (LMTO) [14] method has become very popular for the calculation of the electronic structure for crystalline systems. The LMTO method combines the following advantages: (a) It uses a minimal basis, which leads to high efficiency and makes calculations possible for large unit cells. (b) In this method all elements are treated in the same way, so that atoms with a large number of core states can be considered (say, phases containing d and f metals). (c) This method is very accurate, due to the augmentation procedure which gives the wave function the correct shape near the nuclei. (d) It uses atom-centered basis functions with well-defined angular momentum, which makes the calculation transparent [15]. 3.3.1 Muffin-tin orbitals The crystal is divided into non-overlapping muffin-tin1 spheres surrounding the atomic sites and an interstitial region outside the spheres. Inside the muffin-tin sphere the potential is assumed to be spherically symmetric while in the interstitial region the potential, V M T Z , is assumed to be constant or slowly varying. Because the potential in the interstitial is constant we can shift the energy scale and set it to zero. In the following overview of the method we 1 The picturesque name of muffin-tin derives from the fact that it looks like a pan for cooking muffins. 30 3.3. THE LMTO METHOD consider a crystal with only one atom per primitive cell. Within a single muffin-tin well we define the potential by V (r) − VM T Z , |r| < SM T VM T (r) = (3.13) 0 , |r| > SM T Here V (r) is the spherically symmetric part of the crystal potential. The radii of the muffintin spheres are chosen such that they do not touch each other. In the following S M T is expressed by S. To solve the Schrödinger equation for the muffin-tin potential [−∇2 + VM T ]ψ(ε, r) = (ε − VM T Z )ψ(r) (3.14) one introduces the kinetic energy κ 2 in the interstitial region by κ2 = (ε − VM T Z ) (3.15) For an electron moving in the potential from an isolated muffin-tin well embedded in the flat potential VM T Z , the spherical symmetry can extend throughout all space and the wave functions become ψL (ε, r) = il Ylm (r̂)ψl (ε, r) (3.16) using the convention that r = |r| and r̂ is the direction of r and including a phase factor i l . To obtain basis functions which are approximately independent of energy, reasonably localized, and normalizable for all values of κ2 , Andersen [16] used muffin-tin orbitals. The spherical Bessel functions added to the wavefunction for r < S cancels the divergent part of ψl (ε, k, r) and simultaneously reduce the energy and potential dependence at the tails. Moreover, it incorporates the effects due to the neighbors into the wavefunction so that a minimal basis set of LMTO functions can accurately describe the system [17]. Hence, the muffin-tin orbitals can take the form (r/S)l ψl (ε, r) + Pl (ε) 2(2l+1) , |r| < S l m (3.17) χlm (ε, r) = i Yl (r̂) −l−1 , |r| > S (r/S) where ψl (ε, r) is a solution of the radial Schrödinger equation inside the atomic sphere. Pl (ε) = 2(2l + 1) Dl (ε) + l + 1 Dl (ε) − l (3.18) The potential function and the normalization of ψl (ε, r) are determined by satisfying differentiability and continuity of the basis function on the sphere boundary. Here the term Dl (ε) is the logarithmic derivative of the wave function. The tail of the basis function, i.e., the part outside the muffin-tin sphere is in general introduced as Neumann function, but in Eq. (3.15) the kinetic energy of this tail (known as k 2 ) is simply chosen to be zero. Therefore the Neumann function has a simple form like the above. 31 CHAPTER 3. COMPUTATIONAL TECHNIQUES Figure 3.2: The atomic sphere approximation (ASA) in which the muffin-tin spheres are chosen to have the same volume as the Wigner-Seitz cell, resulting in overlapping spheres. 3.3.2 The LMTO − atomic sphere approximation method In the LMTO-atomic sphere approximation (LMTO-ASA) [18], the muffin-tin spheres are overlapping in such a way that the total volume of the muffin-tin sphere equals the atomic volume. This means that the muffin-tin radius S is equal to the Wigner−Seitz radius S W S 3 . In the ASA, the potential where the total volume per atom is given by V = (4π/3)SW S is also assumed to be spherically symmetric inside each muffin-tin sphere, and the kinetic energy of the basis functions in the interstitial is restricted to be constant, actually zero in the calculation. In order to construct a linear method, the energy dependent terms in the muffin-tin spheres of Eq. (3.17) are replaced by the energy independent function Φ. The function is defined as a combination of radial functions and their energy derivative Φ(D, r) = φl (r) + ω(D)φ̇l (r), (3.19) where ω(D) is a function of the logarithmic derivative. ω(D) should make the energy dependent orbitals χlm (ε, r), defined in Eq. (3.17), continuous and differentiable at the sphere boundary S. The boundary condition is determined as D = −(l + 1). The thus obtained energy independent orbital can now be written as χlm (ε, r) = il Ylm (r̂) Φl (D, r) , |r| < S (r/S)−(l+1) , |r| > S 32 (3.20) 3.4. FULL POTENTIAL METHODS (a) (b) Figure 3.3: (a) The muffin-tin division of space into spheres and interstitial regions. (b) Schematic representation of the wave function inside the sphere (by a radial function) and in the interstitial region (by a Hankel and Neumann function or by a plane-wave). The vertical dotted lines indicate the sphere boundaries. 3.4 Full potential methods All electron methods with localized basis functions, or with more intricate basis sets, such as the linearized augmented plane-wave (LAPW) and LMTO methods are widely used since they are more precise. However, the most accurate all-electron methods can be more computationally demanding than pseudopotential techniques. In the full-potential methods space is divided into two types of regions: non-overlapping spheres surrounding the atomic 33 CHAPTER 3. COMPUTATIONAL TECHNIQUES sites called muffin-tin spheres and region outside these spheres called interstitial region. Since the linearized methods have been derived in terms of matrix elements of the Hamiltonian in a fixed basis, one simply has to calculate matrix elements of the full non-spherical potential in the sphere and the full spatially varying potential in the interstitial. The basis functions are the same in LMTO, LAPW or projected-augmented-wave (PAW) functions which are derived from a spherical approximation to the full potential. However, the spheres merely denote convenient boundaries defining the regions where the basis functions and the potential have different representations. Various calculational schemes differ from each other only in the treatment of the interstitial regions. In the self-consistent calculation one also needs to calculate the potential arising from the density. This necessitates a procedure in which the Poisson equation is solved taking into account the sharply varying charge density inside the spheres. The field inside can be expanded in spherical harmonics and outside the spheres can be represented by smooth functions. 3.4.1 The full potential LMTO method The FP-LMTO calculations [19] are all electron and fully relativistic, without shape approximation to the charge density or potential. The crystal is divided into non-overlapping muffin-tin spheres and interstitial regions outside the spheres. The wave function is then represented differently in these two types of regions. Inside a muffin-tin sphere, the basis functions are as in the LMTO-ASA method, viz. a Bloch sum of linear muffin-tin orbitals expanded by structure constants [φ ν (r) and φ̇ν (r)]. In the interstitial region, Hankel and Neumann functions are used to describe the spatially varying potential. But unlike the ASA (where kinetic energy is resticted to be zero in the interstitial region) the kinetic energy is not a constant. For simplicity, here we only consider a mono-atomic solid and suppress the atomic site index. The κ dependent linear muffin-tin orbitals can now be written as, ψklm (k, r) = χklm (r) + Jklm (r)Sklm,l m (k), (3.21) lm where χlm (r) = il Ylm (r̂) Φ(Dh ,r) −ikhl (κS) Φ(D h ,S) −ikhl (κr) , |r| < S , |r| > S (3.22) and Jklm (r) = il Ylm (r̂) Φ(DJ ,r) Jl (κS)(κS) Φ(D J ,S) Jl (κr) , |r| < S , |r| > S (3.23) Inside the muffin-tin sphere at τ , we can also expand the electron density and potential in spherical harmonics times a radial function, 34 3.4. FULL POTENTIAL METHODS nτ (r)|τ = nτ (h; rτ )Dh (r̂τ ), (3.24) Vτ (h; rτ )Dh (r̂τ ), (3.25) h Vτ (r)|τ = h where Dh are linear combinations of spherical harmonics, Ylm ( r̂). Dh are chosen here because we need an invariant representation of the local point group of the atomic site contained in the muffin tin. The expansion coefficients n τ (h; rτ ) and Vτ (h; rτ ) are numerical functions given on a radial mesh. In the interstitial region, the basis function, charge density, and potential are expressed as Fourier series, ψ(k; r)|I = ei(k+G).r ψ(k + G), (3.26) G nI (r)|I = nG ei(k+G).r , (3.27) VG ei(k+G).r , (3.28) G VI (r)|I = G where G are reciprocal lattice vectors spanning the Fourier space. 3.4.2 The basis set Envelope functions form a suitable basis in interstitial regions. By choosing the appropriate envelope function, e.g., plane waves, Gaussians, and spherical waves (Hankel functions), one can utilize various electronic structure methods (LAPW, LMTO, etc.). The LMTO envelope function is represented as Klm (κ; r) = −κ l+1 l i Ylm (r̂) −h+ l (κr) nl (κr) κ2 ≤ 0 κ2 > 0 (3.29) where nl is a spherical Neumann function and h+ l is a spherical Hankel function of the first kind. The envelope function is singular Hankel or Neumann functions with regards to the sign of the kinetic energy. This introduces a κ dependence for the basis functions inside the muffin-tin sphere through the matching conditions at the sphere boundary. Using variational method, the ground state still has several basis functions with the same quantum numbers, n, l, and m, but different κ 2 . This is called a double-basis approach. The basis can always contain different basis sets corresponding to the atomic quantum number l, but with different principal quantum numbers n. A basis constructed in this way forms a fully hybridizing basis set, rather than a set of separate energy panels. 35 CHAPTER 3. COMPUTATIONAL TECHNIQUES 3.4.3 The LMTO matrix We now introduce a convenient notation for the basis functions: |χi (k) = |φi (k) + |ψi (k), (3.30) where |φ is the basis function inside the muffin-tin spheres and |ψ i (k) represents the tails of basis-function outside the spheres. A wave function Ψkn (k) is then constructed by a linear combination of the LMTO basis functions, χi . The linear combination can be written as |Ψ = Ai |χi (3.31) i The Hamiltonian operator is Ĥ = H0 + Vnmt + VI (3.32) where H0 is the Hamiltonian operator containing the kinetic energy operator and the spherical part of the muffin-tin potential, Vnmt represents the non-spherical part of the muffin-tin potential, and VI is the interstitial potential. Then by using the variational principle for the one-electron Hamiltonian, the LMTO secular matrix follows as [χi (k)|H0 + Vnmt + VI |χj (k) − ε(k)χi (k)|χj (k)]Aj = 0 (3.33) j which can be reduced to 0 1 [Hij + Hij − ε(k)Oij ]Aj = 0 (3.34) j where 0 = φi (k)|H0 |φj (k) Hij (3.35) Oij = φi (k)|φj (k) + ψi (k)|ψj (k) (3.36) and 1 1 = φi (k)|Vnmt |φj (k) + (κ2i + κ2j )ψi (k)|ψj (k) + ψi (k)|VI |ψj (k) (3.37) Hij 2 0 is the spherical muffinwhere |ψj (k) is an eigenfunction to ∇2 with eigenvalue κ2j , Hij tin part of Hamiltonian matrix, Oij is the overlap between the orbitals inside the sphere as 1 contains the corrections to the Hamiltonian mawell as in the interstitial region, and Hij trix coming from the muffin-tin and interstitial regions. The first term in Eq. (3.37) is the non-spherical potential matrix, the next term is the expectation value of the kinetic energy operator in the interstitial region, and the last term is the interstitial potential matrix. 36 3.5. FULL POTENTIAL LAPW METHOD Total energy The total energy for the whole crystal can be expressed as [20] Etot = Tval + Tcor + Ec + Exc (3.38) where Tval and Tcor are the kinetic energy for the valence and core electrons, respectively, E c is the electrostatic energy including electron-electron, electron-nucleus, and nucleus-nucleus contributions, and Exc is an exchange energy term. The kinetic energy is usually expressed as the expectation value of the kinetic energy operator −∇ 2 . According to the eigenvalue equation the expectation value can be expressed as a sum over one-electron energies minus the effective potential energy. The core eigenvalues ε iτ are obtained as an exact solution to the Dirac equation with the spherical part of the muffin-tin potential Etot = occ wnk εkn + μτ kn fiτ εiτ + 1 Zτ j Vc (τj ; 0) + − 2 j 1 n(r) Vc (r) − Vin (r) dr 2 Vc ρ(r)εxc (ρ(r))dr, (3.39) Vc where the integral run over the unit cell [16]. The term with summation over j covers the core states. The density ρ(r) is the total charge density, including valence as well as core electrons. Vin is the input potential obtained from LDA. The Madelung term V c (τ ; 0) describes the Coulomb potential at the nucleus (excluding the Z/r self contribution) and ε xc is the exchange-correlation energy. 3.5 Full potential LAPW method Some of the calculations in the present project have been carried out using the FP-LAPW program package WIEN97 and WIEN2K [21]. The LAPW method is a very accurate calculational scheme for electronic-structure investigations. This approach is characterized by the use of a basis set which is especially adapted to the problem. The method is basically derived from the augmented-plane-wave (APW) approach. The construction of APW developed by Slater is motivated by the fact that near an atomic nucleus the potential and wavefunctions are similar to those in an atom; strongly varying, but nearly spherical. Conversely, between the atoms both the potential and wavefunctions are smoother. Accordingly, space is divided into two regions and different basis expansions are used in these regions: radial solutions of Schrödinger’s equation inside non-overlapping atom-centered spheres and plane-waves in the remaining interstitial regions. ϕ(r) = r ∈ interstitial lm Alm ul (r)Ylm (r) r ∈ inside − sphere 1 Ω1/2 i(G+k)r G CG e 37 (3.40) CHAPTER 3. COMPUTATIONAL TECHNIQUES where ϕ is the wave function, Ω the cell volume and u l the regular solution of the Eq. 3.40. Here CG and Alm are expansion coefficients, El is a parameter (introduced equal to the band energy) and V is the spherical component of the potential inside the sphere: l(l + 1) d2 + + V (r) − E (3.41) l rul (r) = 0 dr 2 r2 The particular choice of these functions was motivated by Slater who noted that planewaves are the solutions of Schrödinger equation for a constant potential, while the radial functions are solutions for a spherical potential, provided that E l is equal to the eigenvalue. This approximation known as muffin-tin approximation is commonly used in APW codes and is very good for close-packed (like fcc and hcp) materials. The dual representation defined by Eq. 3.40 is not guaranteed to be continuous on the sphere boundaries, as it should be, for the kinetic energy to be well defined. Therefore a constraint is imposed in the APW method, by defining the A lm in terms of CG through the spherical harmonic expansion of the planewaves. The coefficient of each lm component is matched at the sphere boundary. Thus, − Alm = 4φil CG jl (|k + g|R)Ylm (k + G) 1/2 Ω ul (R) G (3.42) where the origin is taken at the center of the sphere and R is the sphere radius. Thus the A lm are completely determined by the plane-wave coefficients C G and the energy parameters El . The individual functions which are labeled by G and consist of single plane-waves in the interstitial matched to radial functions in the spheres are the augmented plane-waves (APWs). 3.5.1 The LAPW basis and its properties In the LAPW method, the basis functions inside the spheres are linear combinations of a radial function ul (r)Ylm (r) and their energy derivatives. The u l are defined with a fixed E l . The energy derivative u̇l (r)Ylm satisfies − l(l + 1) d2 + + V (r) − E r u̇l (r) = rul (r) l dr 2 r2 (3.43) in the non-relativistic case. These functions are matched to the values and derivatives of the plane waves on the sphere boundaries. Plane waves augmented in this way are called LAPW basis functions. In terms of this basis the wavefunctions, 1 i(G+k)r r ∈ interstitial G CG e Ω1/2 (3.44) ϕ(r) = lm [Alm ul (r) + Blm u̇l (r)]Ylm (r) r ∈ inside − sphere where the Blm are coefficients for the energy derivatives analogous to the A lm . The LAPWs are plane waves in the interstitial region of the unit cell, and they match the numerical radial 38 3.6. PSEUDOPOTENTIAL METHOD functions inside the spheres with the requirement that the basis functions and their derivatives are continuous at the boundary. In this method no shape approximations are made and consequently such a procedure is often called "full-potential LAPW" (FP-LAPW). The LAPW method has more advantages than the APW method. In the former, accurate energy bands (at a given k point) are obtained with a single diagonalization, while in the APW method the diagonalization is needed for each band. Moreover, the LAPW basis has more flexibility inside the spheres, i.e., two radial functions instead of one. This means that there is no difficulty in treating non-spherical potentials inside the spheres; although the optimum value of El is not known a priori, the flexibility arising from u̇l allows an accurate solution. There is however a price to be paid for this flexibility. This arises from the requirement that the basis functions should have continuous derivatives. Higher plane wave cut-offs are required to achieve a given level of convergence. In the WIEN2K package the total energy is calculated according to the Weinert scheme [22]. The convergence of the basis set is controlled by the cut-off parameter R mt Kmax (determining the size of the matrix of the system), which usually assumes values between 6 and 9. The Rmt represents the smallest of all atomic sphere radii in the unit cell and K max is the magnitude of the largest K vector (plane-wave cut-off). There is a quantitative difference between the LAPW and LMTO approaches in the requirements of the full potential. Since the minimal basis for LMTO only involves functions with lmax given by the actual angular momenta or the primary states making up the band, only angular momenta up to 2lmax are relevant. However, for the LAPW methods, much higher angular momenta in the wavefunctions are required (typically lmax ≈ 8 to 12 for accurate calculations) to satisfy the continuity conditions accurately. The difference results from the fact that, the LAPW basis is much larger; in order to represent the interstitial region accurately, many plane waves are required. 3.6 Pseudopotential Method In 1934, Fermi first introduced the concept of pseudopotential. He interpreted the measured optical spectra of alkali atoms arising from transitions to high-lying electronic energy levels using the so-called pseudopotential and argued that for high-lying states the oscillations of the wave function near the atomic core played a very small role. Therefore he built a potential that gave a nodeless pseudo-wave-function which had the correct large-distance behavior. In most materials the core electrons do not contribute to the bonding, but only their absolute energy is affected by the average electrostatic potential in the vicinity of the core (core level shift). A fundamental idea is therefore the “frozen-core approximation”. The pseudopotential approximation treats each nucleus plus its core electrons as a “frozen core” that does not change in response to changes in its environment. The interactions of the valence electrons with this core are then described by a pseudopotential, usually constructed from all-electron calculations to reproduce the eigenvalues, and the wavefunctions outside the core. The core electrons are calculated for a reference configuration (in general, 39 CHAPTER 3. COMPUTATIONAL TECHNIQUES spherical) and are kept fixed thereafter. The wave functions for the valence electrons are treated (pseudized) so as to give the same energy levels as the all-electron wavefunctions. The pseudo wavefunctions differ from the all-electron wavefunctions only inside a region around the nucleus and are constructed to be nodeless. Nodeless pseudo-wavefunctions reduce the number of required plane waves considerably. It is implicit within the pseudo potential approach that the exchange-correlation potential, V xc , like the direct Coulomb potential is separable into a core part and a valence part. The main advantage of the pseudo potential method is that one does not need the complicated all-electron wave functions but only the pseudo wavefunctions which are tailored to be well-behaving numerically. Another advantage is that one needs to calculate the properties of ion only once in an environment such as a free atom and use it throughout all other DFT calculations. The frozen-core approximation allows one to transfer the properties of the free atom to an atom bound in a solid. One of the most widely used implementations of DFT is the so-called plane wave pseudopotential method in which the KS wave functions are expanded in a basis of plane waves. Plane wave basis sets offer many advantages in DFT calculations for solids including completeness, unbiased representation, and arbitrarily good convergence accuracy. They also allow for straight forward mathematical formulation and implementation, which is convenient for the calculation of Hellmann-Feynmann forces in DFT perturbation calculations and for linear response calculations [23]. Having determined the pseudopotential, the total structural energy E str can be evaluated. The contributions to E str include the Madelung core-core energy, the electron-core energy, the kinetic energy of the electrons (which can be evaluated from the pseudopotential and wave functions), the electron-electron Hartree energy, and the exchange-correlation energy (which can be evaluated using the charge density). The input is the atomic number for each constituent atoms and the crystal structure. For a given structure, the volume for which Estr has a minimum that determines the lattice constants, and the curvature yields the bulk modulus. Although molecular dynamics schemes have been developed and are improving, at present one has to generally rely on the comparison of candidate crystal structures to predict or explain properties of different solid phases. Future molecular dynamics techniques will likely allow the predictions of new non-equilibrium solid phases with interesting and useful properties. The fact that the total-energy pseudopotential method could predict the existence of a solid phase and its ground-state properties gave a significant boost to the research in this field [24]. The added claim that only the atomic number, atomic mass, and candidate crystal structures are used as input provided credence for the proposition that the total-energy pseudopotential approach is a first-principles method that could serve as a useful standard model of solids. 40 3.7. THE PROJECTED AUGMENTED WAVE (PAW) METHOD 3.7 The projected augmented wave (PAW) method In the pseudopotential methods a potential and its corresponding pseudo wave functions are constructed to reproduce the atomic scattering properties in an energy window around the atomic eigenvalues. They are then used as input parameters to the many-particle DFT calculations. The PAW method is in principle a frozen-core all-electron method that aims at adding the advantages and accuracy of all-electron methods to the more simple and computationally less demanding pseudopotential method. Blöchl [25] developed the projected-augmented wave method (PAW) by combining ideas from the pseudo potential and linear augmented-plane-wave (LAPW) methods. The PAW method starts from a simple linear transformation that connects the exact valence wave function |ψ to a pseudo (PS) wavefunction |ψ̃ which is expanded into plane waves, ˜ pN,i |φN,i ˜ |ψ̃ + |φN,i p̃N,i |ψ̃ (3.45) |ψ = |ψ̃ − N,i N,i All quantities related to the PS representation of the wave function are indicated by the tilde symbol. The φ are local wave functions, the index N goes over all sites, and i over the quantum numbers n, l, and m. The p˜i are localized projector functions that have to fulfill the condition |φ̃p̃i | = 1. (3.46) i Defining the character cN,i of an arbitrary wave function ψ̃ at the atomic site N as cN,i = p̃N,i |ψ̃, (3.47) the pseudo- and all-electron wavefunctions at an atomic site N can be easily reconstructed from the plane-wave expanded pseudo wave functions as, |φ̃N,i cN,i (3.48) |ψ̃N = i and |ψN = |φN,i cN,i . (3.49) i The variational quantities that need to be determined during the ground-state calculation are the PS wave function ψ̃. However, contrary to the “simple" pseudopotential methods the operators A representing physical quantities need to be consistently extended to their all-electron forms, |p̃N,i φN,i |A|φN,j − φ̃N,i |A|φ̃N,j p̃N,j |. (3.50) Ã = A + N,i,j The above equation is valid for local and quasi-local operators such as the kinetic energy. The valence-only PAW method is implemented in the program package VASP [26]. Its results are almost identical to the most accurate DFT calculations which are based on the FP-LAPW method. 41 CHAPTER 3. COMPUTATIONAL TECHNIQUES 3.7.1 Charge density The charge density at a point r in space is composed of three terms: ρ(r) = ρ̃(r) + ρ (r) − ρ̃ (r) (3.51) The soft pseudo-charge density ρ̃(r) is the expectation value for the real-space projection operator |rr| on the pseudo-wave functions. ρ̃(r) = fn Ψ̃n |rr|Ψ̃n (3.52) n The on-site charge densities ρ (r) and ρ̃ (r) are treated on a radial support grid. They are given as : ρ (r) = fn Ψ̃n |p˜i φi |rr|φj p˜j |Ψ̃n = nij φi |rr|φj (3.53) n where nij is the occupancy of each augmentation channel (i, j) which is obtained from the pseudo-wave functions on applying the projector functions: nij = n fn Ψ̃n |p˜i p˜j |Ψ̃n . Similarly for ρ̃ (r): ρ̃ (r) = fn Ψ̃n |p˜i φ̃i |rr|φ̃j p˜j |Ψ̃n = nij φ̃i |rr|φ˜j (3.54) n We will focus on the frozen-core case, where ρ̃, ρ̃ , and ρ are restricted to valence quantities. Besides that, we introduce four quantities that will be used to describe the core charge density: ρc , ρ̃c , ρZc , and ρ̃Zc . ρc denotes the charge density of the frozen core all-electron wave function at the reference atom. The partial-core density ρ̃ is introduced to calculate the nonlinear core corrections. ρZc is defined as the sum of the point charge of the nucleus ρ z and the frozen core AE charge density ρ c : ρZc = ρz + ρc . The pseudized core density is a charge distribution that is equivalent to ρ Zc outside the core radius and with the same moment as ρ Zc inside the core region. 3 ρZc (r)d r = ρ̃Zc (r)d3 r (3.55) Ωr Ωr The total charge density ρ T [27] is decomposed into three terms: ρT = ρ + ρZc = (ρ̃ + ρ̂ + ρ̃Zc ) + (ρ + ρZc ) − (ρ̃ + n̂ + ñZc ) = ρ˜T + ρT − ρ̃T (3.56) A compensation charge ρ̂ is added to the soft charge densities ρ̃ + ρ̃ Zc and ρ̃ + ρ̃Zc to reproduce the correct multiple moments of the AE charge density ρ + ρZc in each augmentation region. Because ρ Zc and ρ̃Zc have exactly the same monopole −Zion (the charge of 42 3.7. THE PROJECTED AUGMENTED WAVE (PAW) METHOD an electron being new +1), the compensation charge must be chosen such that ρ̃ +ρ̂ has the same moments as the AE valence-charge density ρ within each augmentation sphere. 3.7.2 Total energy The final expression for the total energy can also be split into three terms: E(r) = Ẽ(r) + E (r) − Ẽ (r) (3.57) where Ẽ(r), E (r), and Ẽ (r) are given by Ẽ(r) = n 1 fn Ψ̃n | − Δ|Ψ̃n + Exc [ρ̃ + ρ̂ + ρ˜c ] + EH [ρ̃ + ρ̂] + 2 vH [ρ̃Zc ][ρ̃(r) + ρ̂(r)]dr + U (R, Zion ) (3.58) where U (R, Zion ) is the electrostatic energy of the point charges Z ion in an uniform electrostatic background. E (r) = ij 1 nij φi | − Δ|φj + Exc [ρ + ρc ] + EH [ρ ] + 2 vH [ρ̃Zc ]ρ (r)dr (3.59) where vH [ρ̃Zc ]ρ (r)dr is the electrostatic interaction between core and valence electrons and EH is electrostatic energy 1 1 EH [ρ] = (ρ)(ρ) = 2 2 E˜1 (r) = ij + dr dr ρ(r)ρ(r ) |r − r | (3.60) 1 nij φ̃i | − Δ|φ̃j + Exc [ρ̃ + ρ̂ + ρ̃c ] + EH [ρ̃ + ρ̂] 2 vH [ρ̃Zc ][ρ̃ (r) + ρ̂(r)]dr (3.61) The overlining signalizes that the corresponding terms must be evaluated on the radial grid within each augmentation region. 43 CHAPTER 3. COMPUTATIONAL TECHNIQUES 3.8 Brillouin zone integration In order to determine the charge density and other quantities such as total energy, forces etc. it is necessary to evaluate sums over the occupied states. As discussed in Sec.3.1, for crystals this can be done over the Brillouin zone and by the application of crystal symmetry, can be reduced to integrals over the irreducible wedge of the zone (IBZ). Following the variational principle (minimizing the total energy), and the Pauli-exclusion principle, eigenstates with eigenvalues εi (k) are filled starting from the energetically lowest eigenvalue. The energy of the highest filled eigenstate is called the Fermi energy (E F ). The Fermi energy is given from εF D(ε)dε, (3.62) N= −∞ where N is the number of valence electrons and D(ε) is the density of the states (DOS), dS 2 (3.63) D(ε) = 3 8π S(ε) |∇ε(K)|. The integration is carried out all over a surface of constant energy, S(ε), in the IBZ. The one-electron states most relevant for physical properties are those with energies around the Fermi level. These states are important for the stability of the crystal structure, transport properties, magnetic susceptibility, etc. The integrals are necessarily calculated numerically using wavefunctions and eigenvalues at a finite number of k points in the zone. The two commonly used methods are briefly discussed below. 3.8.1 Special points method In this method integrations are performed as weighted sums over a grid of representative k points. The locations of the representative (or special) points and the corresponding weights are independent of the band energies, and are chosen to yield optimum convergence for smooth functions. This method is well suited for insulators. In metals, bands intersect the Fermi level leading to discontinuities in the occupation and therefore in the integrands on the Fermi surface. In order to overcome this difficulty an artificial broadening of the Fermi surface is used. 3.8.2 Tetrahedron method In the tetrahedron approach, the zone is divided into tetrahedra and the band energies and wave functions are computed at k points on the vertices. This is particularly useful because tetrahedra can be used to fill all space for any grid. The band energies are interpolated linearly between the vertices, and this interpolation is used to determine the Fermi energy. Each band at each k point is then assigned a weight based on the volume of the 44 3.8. BRILLOUIN ZONE INTEGRATION tetrahedron for which it occurs below EF , and the charge density is calculated by summing the individual contributions with these weights. The tetrahedron method is very important in calculations on transition metals, rare earths etc., where there are exquisite details of the Fermi surfaces that must be resolved. 45 CHAPTER 3. COMPUTATIONAL TECHNIQUES 46 CHAPTER 4 Ground-state Properties and their Analyses The end of all our exploration will be to arrive where we started. T.S. Eliot T he properties of matter are usually determined by the electronic ground and excited states. Ground-state properties include: cohesive energy, equilibrium crystal structure, phase transitions between different structural arrangements, elastic constants, charge density, magnetic order, static electric and magnetic susceptibilities, etc. Since typical energy scales for electrons are much greater than those associated with the degrees of freedom for the more massive nuclei, the lowest energy ground state of the electrons determines the structure and low-energy motions of the nuclei. The vast array of forms of matter - from the hardest diamond to soft lubricants like graphite or the many complex crystals formed by the elements of the Periodic Table - are largely manifestations of the ground-state of the electrons involved. 4.1 Structural stability and Phase transitions In the area of phase-stability and phase-diagram prediction, first-principles calculations have made an impact on the understanding of real materials. The equation of state as a function of pressure and temperature is perhaps one of the most fundamental relations in condensed matter. The stable structure at a given pressure (P ) and temperature (T ) determines all the other properties of the material. The total energy (E) at T = 0 K as a function of the volume (Ω) is the most convenient quantity for theoretical analysis because it is quite straightforward to carry out electronic structure calculations at fixed volume. In other words, volume is a convenient “knob” that can be tuned to control the system theoretically. Comparison of theoretical and experimental volume is one of the touchstones of “ab initio” electronic-structure research. CHAPTER 4. GROUND-STATE PROPERTIES AND THEIR ANALYSES The total energy E and Ω per unit cell, together with P and bulk modulus B are related by the equations, dE dP d2 E E = E(Ω), P = − , B = −Ω = Ω 2. (4.1) dΩ dΩ dΩ One has to first determine the equilibrium volume of the cell where E is minimum or P = 0, and bulk modulus (B) for the zero-pressure crystal structure. The most commonly used approach (and that used in this project) is, to calculate E for several different Ω values, and fit these to an analytic function, e.g., the Murnaghan equation of state [28, 29, 30] or the socalled universal equation of state [31] (used here). The minimum gives the corresponding equilibrium volume and total energy, and the second derivative, the bulk modulus. The major challenge for computational materials science is the prediction of crystal structure. While the properties of a material in a given structure can be predicted, it is still very difficult to demonstrate that a particular chosen structure will be stable or even metastable. With all the sophistication of first-principles theory, structure prediction still has to be approached with brute (but ineffective) force. To “predict” the structure of a compound, we have to compute, at best the total energy for a few “reasonable” candidate arrangements and then proclaim the one with the lowest total energy to represent the ground-state structure. While such an approach may be reasonable when working on well-known systems, it may be of little benefit when dealing with novel or complex multicomponent materials. In a substantial part of this project we have, e.g., studied structural stability and predicted crystal structures for a series of mixed-valence chromium oxides which turned out to be one of the most demanding projects dealt in this thesis. The actual structures considered for the prediction and detailed results are given in Publications VI to IX. 4.2 Electronic Structure As outlined in Chapter 2, the electronic structure of materials determines ground-state properties such as electrical conductivity. An electronic structure is often visualized by a band-structure plot. A band is the track of an eigen value in reciprocal space. 4.2.1 Classification of materials Based on the intrinsic electronic structure and the filling of bands, materials can be classified as metals, insulators, semiconductors, and half metals. Metals Metals are characterized by a band structure in which the highest occupied band (the valence band; VB) is partially filled. The highest occupied energy level is called the Fermi level (EF ). Metals usually have some vacant levels just below the EF whereas some occupied levels occur above EF at T = 0 K. Since metals do not have to be overcoming excitation gaps, the band electrons in singly occupied states close to the E F are able to move around 48 4.2. ELECTRONIC STRUCTURE relatively freely and these electrons are responsible for the conductivity of metals. Insulators The VB of an insulator is completely filled. The highest energy level of VB is separated from the lowest energy level of conduction band (CB) by a forbidden energy gap (E g ) of the order of some 5 eV. Even at appreciable temperatures very few electrons from the VB have sufficient thermal energy to be promoted to the CB, hence insulators have zero or negligible conductivity. Semiconductors Semiconductors have a similar band structure to insulators, but the E g is smaller, say, in the range of 0.2 to 2.0 eV. At low temperatures a few electrons have sufficient thermal energy to be promoted to CB and hence create conductivity in an electric field. However, the excitation process is described by an exponential function of temperature and the conductivity may accordingly reach appreciable values at higher temperatures. It should be noted that insulators are really special cases of semiconductors, distinguished by a much larger size of Eg . Note that for many purposes the Fermi level (E F ) of insulators and semiconductors are postulated to be located midway between VB and CB. Half metals Half metals constitute an unique class of magnetic materials in which one of the spin channels (usually postulated as the majority-spin channel) has metallic character and the other spin channel has insulating (semiconducting) character with a distinct band gap extending from the top of the highest filled energy level to the lowest empty energy level (at 0 K). 4.2.2 Density of states An important description of the electronic structure for many purposes is provided by the density of states (DOS) which is another way to visualize and analyze the electronic structure. In a DOS diagram the abscissa axis is usually chosen as energy and the ordinate axis is the number of eigenvalues (states) at a particular energy level. The energy scale is conveniently chosen so that the E F is located at zero energy. Ω 1 δ(i,k − E) = dkδ(i,k − E). ρ(E) = Nk (2π)d BZ (4.2) i,k Assuming independent-particle states, and taking i,k as the energy of an electron, Eq.4.2 provides the number of independent-particle states per unit energy. The DOS provides us with the ground-state electronic structure of a given material and helps us to classify materials in the categories metals, insulators, semiconductors and half metals. For example, Fig. 4.1 presents the electronic structure of Ca 3 Co2 O6 in various magnetic configurations. In the ground-state ferrimagnetic configuration, Ca 3 Co2 O6 has a distinct 49 CHAPTER 4. GROUND-STATE PROPERTIES AND THEIR ANALYSES Ferrimagnetic; metal 10 0 −10 Ferromagnetic; half−metal −1 −1 DOS (states eV f.u. ) 10 0 −10 Paramagnetic; insulator 10 0 −10 −8 −6 −4 −2 0 2 4 6 Energy (eV) Figure 4.1: Total density of states plots for Ca3 Co2 O6 in different magnetic configurations. number of states at the EF implying metallic character. On the other hand, in the higherenergy ferromagnetic configuration, the majority-spin channel still exhibits electronic states at EF whereas the minority-spin channel shows an energy gap of around 1.15 eV, implying half-metallic character. Further, in the paramagnetic configuration, both majority- and minority-spin channels show gaps of around 0.29 eV, indicating semiconducting behavior. It is worthwhile to note here that we can also extract excited state properties of a material from the DOS and derived quantities thereof. 4.3 Bonding Characteristics The stable structures of solids are most naturally considered in terms of the electronic ground state which determines the bonding of nuclei. The lowest energy state of the electrons determines the location of the nuclei in space and, conversely, the spatial structure of nuclei provides the external potential that determines the Schrödinger equation for the electrons. When atoms combine to form a solid, the repulsion between the positive ion cores of 50 4.3. BONDING CHARACTERISTICS the atoms is overcome by the attractive forces of the valence electrons that holds the material together. While the ion cores occupy fixed positions (in the structural framework) the valence electrons “whiz” around and between them, forming a kind of electrostatic glue known as “bonding”. 4.3.1 Types of bonding Bonding in materials is classified according to the four idealized types of bond. Ionic bonding Ionic bonding is found in compounds formed by combination of elements with a large difference in electronegativity. This type of bonding occurs when some of the valence electrons from one atomic species are donated wholesale to another atomic species. The ionic systems can be characterized by charge transfer to form closed-shell ions, often leading to structures with the larger sized anions in close-packed arrangements and small cations in intermediate positions to maximize Coulomb attraction (or minimize anion-anion repulsion). Unlike the other bonding types the idealized ionic bonding can be understood and rationalized in terms of the Coulomb law from classical physics. The cohesive energy for an idealized ionic compound is completely determined by the attractive and repulsive forces between the ions. Covalent bonding Covalent bond can only be accounted for in terms of quantum mechanical concepts. This type of bonding involves a complete change of electronic states from, say, isolated atom (or ion) to well-defined bonding states in solids. Covalent bonds are directional bonds that result from the formation of localized electronic states with pairing of electrons. One of the main requirements for a covalent bond to be formed is the presence of degenerate energy levels of the constituents so that they can be shared between the constituents. (The essential feature is pairing process whether or not a pair of electrons are involved). Metallic bonding Metallic bonding is visualized as itinerant conduction electrons spread among the ion cores forming homogeneous electron gas. Unlike in covalent bonds, the electronic states are essentially delocalized but the crucial features of the covalent bonding (viz. the paired distribution of electrons) is the same. Metals are usually good conductors because there is no energy gap for electronic excitation, when the bands are partially filled they can easily accept different number of electrons which can drift easily between the ion cores. This also enables metals to form alloys among atoms with different valency. Van der Waals bonding Van der Waals bonding is sometimes referred to as closed-shell bonding and may be exemplified by rare gas and molecular solids. Phases with van der Walls bonding have electronic states qualitatively similar to those of free atoms, weak van der Waals attraction being bal51 CHAPTER 4. GROUND-STATE PROPERTIES AND THEIR ANALYSES (b) 8 6 6 4 4 2 2 Energy (eV) Energy (eV) (a) 8 0 0 -2 -2 -4 -4 -6 -6 -8 -8 g X M g Z R A M g X M g Z R A M Figure 4.2: Illustration of (a) majority-spin and (b) minority-spin bandstructures of one type of Mn in the ferrimagnetic insulator YBaMn2 O5 . The dz2 orbital is highlighted with fat band notation. anced by repulsion from orbital overlap. Hydrogen bonding, which is thought to be crucial within many molecules and of important biological activity, is not considered here. The bonding in a real material is, in general, a combination of all three main types described above. For example, in a metal there can be directional covalent bonding as well as contributions of ionic character due to local charge transfer. In this thesis, we will see a generous number of systems displaying an admixture of the different types of bonding. The challenge for electronic-structure theory is to provide universal methods that can accurately describe real systems. A theoretical method must not be limited to any particular type of bonding, otherwise it would be rather unproductive. The theory should provide understanding, and not merely numerical values for more or less well-chosen parameters. Different analytical tools (based on DFT) used to visualize and characterize different types of bonding in this thesis are described below. 4.3.2 Partial density of states Band structures and density of states are common tools for investigating the physical properties of solids. In order to obtain a more local picture of bonding, one can use projected band structure (“fat bands” which display the contribution of one given atom (or one given atomic orbital) in each band for selected directions in reciprocal space (see for example, Fig. 4.2 where dz 2 orbital in one of the Mn atoms in YBaMn2 O5 is shown as fat band). DOS 52 4.3. BONDING CHARACTERISTICS 10 8 Ba 8 O 4 Energy (eV) 0 −4 −8 −12 −16 −20 −10 (a) −5 0 5 10 10 Si O 8 6 6 4 4 2 2 0 0 −2 −2 −4 −4 −6 −6 −8 −8 −10 −5 (b) 0 5 10 Density of states (states eV −1 15 Be −10 −0.5 0 (c) O 0.5 1 1.5 2 −1 atom ) Figure 4.3: Site-decomposed density of states plots for (a) ionic BaO, (b) covalent SiO2 , and (c) semi-covalent BeO. The horizontal dotted line marks (EF ). The region below EF is the valence band and above EF is the conduction band. plots, on the other hand, allow one to calculate atomic gross contributions to the bonding in the whole Brillouin zone. Since the materials studied in this project are mostly multicomponent with large number of atoms, analysis of their electronic structure by means of “fat bands” becomes cumbersome. Hence we have mainly preferred DOS analysis. The site-projected DOS gives an overview picture of the nature of the bonding between the constituents of a solid. By studying the electronic DOS decomposed according to site and angular momentum one can, in principle, distinguish between ionic and covalent bonding in a compound. If the bonding is strongly ionic, there is little mixing of states from one atom into states of other atoms [see, Fig. 4.3a, where the Ba and O states in BaO are well separated from each other]. If the bonding is primarily covalent, the states of different atoms are mixed together and one would expect to find similar decomposed state densities for all sites [32]. When two atoms interact, their states hybridize with one another to form bonding and antibonding states. Only when the valence states of the constituents are approximately degenerate, does a strong covalent hybridization occur. For SiO 2 in Fig. 4.3b one can see the Si and O states in the same energy region, indicating energetic degeneracy and hence, the covalent interaction. The hybridization between the d electrons of the transition metal with the s and p electrons of the main group elements lead to sp-d bonding and antibonding hybrids, as well as nonbonding d states. Filling of bonding orbitals increases bond strength, filling non-bonding orbitals has little effect, whereas filling antibonding orbitals reduces the 53 CHAPTER 4. GROUND-STATE PROPERTIES AND THEIR ANALYSES 2 1 0 Ba−O −1 −2 COHP 0 −1 Si−O −2 0 Be−O −0.2 −0.4 −8 −6 −4 −2 0 2 4 6 8 10 Energy (eV) Figure 4.4: Crystal orbital Hamiltonian population plotted for BaO, SiO2 and BeO. The vertical dotted line indicates the Fermi level. bond strength. In Fig. 4.3c we display the DOS for the semi-covalent case BeO which exhibits mainly covalent bonding with a woof of ionic bonding interaction. One of the main tasks of this project has been the study of mixed-valent transition-metal oxides. In order to determine the actual valence states of elements and thereby explore the difference between formal and actual valence states, orbital-decomposed DOS is particularly useful. The orbital-projected DOS provides the occupation of different orbitals with respect to energy. Hence the higher energy orbitals which lead to orbital ordering can be explored (see various publications of this thesis). 4.3.3 Crystal-orbital-Hamiltonian-population (COHP) plot Another useful tool to distinguish bonding, antibonding, and nonbonding interaction between atoms is the crystal-orbital population. According to this COHP concept, negative COHP values indicate bonding, positive values antibonding, and zero COHP together with finite DOS values suggests nonbonding states. COHP is a quite meaningful way to measure the effective strength of bond interactions. It is calculated by weighing the crystal-orbital54 4.3. BONDING CHARACTERISTICS overlap-population with crystal-orbital eigenvalues. Since the latter is less basis-set dependent, COHP should be appropriate in cases with highly degenerated systems. A detailed description of the COHP method can be found in Ref. [33]. The COHP contours should reflect the number of states in a particular energy interval. The integrated COHP (ICOHP) up to the E F represents the total overlap population of the bonds concerned and this can be taken as a measure of bond strength. For example the ICOHP values (from Fig. 4.4) for BaO, SiO2 , and BeO are 0.54, 2.08, and 1.77, respectively. It should be noted that COHP analysis provides the location of bonding, antibonding, and nonbonding electrons. In order to establish the nature of bonding, COHP should be combined with site-decomposed DOS and other bonding-analysis tools. 4.3.4 Charge-density plot The electron density ρ(r) plays a fundamental role in the theory and understanding of systems comprised of electrons and nuclei. Since it is the fundamental quantity in the DFT calculations, an understanding of different bonding can be obtained by plotting the charge density distribution in real space. Fig. 4.5a depicts a typical example of ionic bonding in NaCl; Na+ exhibits reduced charge density whereas Cl − rules over the enhanced charge density. Fig. 4.5b reproduces covalently bonded Si with significant charge density mid way between the Si atoms. In metallic Al charges are seen to be homogenously distributed in the interstitial region (Fig. 4.5c). The charge density is in principle, an indicator for the chemical bonding in a given system, but comes normally out as rather featureless, with charge maxima around the atoms, similar to the charge density for overlapping free atoms. Moreover, it gives the overall charge density including contributions from non-bonding electrons. Hence, one needs additional tools for analysis of the bonding character in the real materials. 4.3.5 Charge-transfer plot If one now (instead of charge density) displays the difference between the electron density of the compound and the electron density of the constituent atoms (viz. difference between the crystal density and that of a sum of superimposed neutral spherical atoms), one obtains an impression of how electrons are shifted around when the solid is formed. This allows one to see how the actual chemical bond is formed in the real space. Mathematically the charge-transfer density is the self-consistent electron density of a solid in a particular plane (ρcomp. ), minus the electron density of the corresponding free atoms (ρ f.a. ) in an identical structural arrangement, Δρ(r) = ρ(r)comp. − ρ(r)f.a. , (4.3) which allows one to visualize how electrons are redistributed in a particular plane of the structure compared to free atoms. 55 CHAPTER 4. GROUND-STATE PROPERTIES AND THEIR ANALYSES Na Cl Al Cl Al 0.4 0.3 Cl Na Na Si Si Na Cl Na 0.1 Cl Al Al 0.0 (c) (b) (a) 0.2 Al Si Si Cl Si Al Cl Al 0.10 0.05 Na Cl Na Si Si Na Cl Na −0.05 Cl Al Al −0.10 (f) (e) (d) 0.00 Al Si Si Cl Si Al Cl Al 0.8 0.6 Na Cl Na Si Si Si Cl Na (f) Si 0.4 Al 0.2 Si Cl Al Al 0.0 (h) (g) Figure 4.5: Charge-density plots for (a) ionic NaCl, (b) covalent Si, and (c) metallic Al. Charge transfer and electron localization function (ELF) plots are shown in the same order for the above materials in (d), (e), (f) and (g), (h), (i), respectively. Fig. 2(d−f) shows the charge transfer in ionic NaCl, covalent Si, and metallic Al, respectively. The negative charge-transfer around Na and positive charge-transfer around Cl indicate the transfer of charges from Na to Cl while forming ionic bonding. On the other hand, in the Si case charge has been transferred to the mid-way region between the Si atoms. An experimental charge difference plot based on scattering by x-rays and high-energy electrons [34] has been found to provide a fully comparable picture with theoretical chargetransfer plot. This suggests that the charge transfer plot may be a very valuable tool to 56 4.3. BONDING CHARACTERISTICS visualize bonds, in particular covalent bonds. In metallic Al, we can see that Al has lost electrons to the interstitial regions. Unlike the other two types of bonding, the directionalcharacter of covalent bonding is clearly exposed from charge-density and charge-transfer plots. In addition, attention may be drawn to the charge difference plotted between LiCr 3 O8 and Cr3 O8 in the same structural arrangement (Fig. 8 in Paper.VII). Such plots have proved very useful to analyze the effect of Li-intercalation in Cr3 O8 , viz, changes in the lattice, bonding character etc as Li enters the Cr 3 O8 lattice. Such an analysis throws some light on the usefulness of LiCr 3 O8 and Cr3 O8 as cathode materials in the rechargeable Li-ion batteries. 4.3.6 Electron-localization function ELF provides a measure of the local influence of Pauli repulsion on the behavior of electrons and permits the mapping in real space of core, bonding and non-bonding regions in a crystal [35]. ELF is a ground-state property which discriminates between different kinds of bonding interaction for the constituents of a solid [35, 36, 37]. In the implementation for DFT, this quantity depends on the excess of local kinetic energy t p originating from the Pauli principle. (4.4) ELF = {1 + [tp(r) /tp,h (ρ(r))]2 }−1 where: tp = τ − 1/8[(∇ρ)2 /ρ] (4.5) is the Pauli-kinetic-energy density of a closed-shell system. (∇ρ) 2 /(8ρ) is the kinetic energy √ density of a bosonic-like system, where orbitals are occupied proportional to ρ. tp is always positive, and for an assembly of fermions, it describes the additional kinetic energy density required to satisfy the Pauli principle. The total electron density (ρ) ρ= n |ψi |2 (4.6) i as well as the kinetic energy density(τ ) τ = 1/2 n |∇ψi |2 (4.7) i are computed from the orbitals ψ i , the index i running over all occupied orbitals. According to Eqn. 4.4, the ELF takes the value one either for a single-electron wave function or for a two-electron-singlet wave function. In a many-electron system ELF is close to one in regions where electrons are paired such as in covalent bonds, or for lone electrons (dangling bonds) while the ELF is small in regions with low density of electrons. In a homogeneous electron gas ELF equals 0.5 at any electron density, and ELF values of this order in homogeneous systems indicates regions where the bonding has metallic character. The ELF 57 CHAPTER 4. GROUND-STATE PROPERTIES AND THEIR ANALYSES distribution for the typical examples of bonding discussed above are shown in Fig. 4.5(g−i). For the NaCl case ELF is around 0.8 at the Cl site and only a non significant ELF value is found at the Na site, thus clearly reflecting ionic bonding. In the Si case, a ELF value just below 1 is found where the shared electrons are located between the Si atoms. In the Al case, maximum values of ELF∼0.5 are found in the interstitial region where the delocalized electrons rule. In addition to these tools, bonding interaction has been analyzed with the help of concepts like “atoms-in-molecule´´ of Bader [38] and Born-effective charges [39, 40]. These method provide a somewhat quantitative measure of charges present in each atomic site in a lattice. From the thus calculated values we can draw conclusions on nature of bonding as well as valence states of individual constituents. A brief description of these methods and the resulting analysis are dealt with in Publications IV and XI, respectively. 58 CHAPTER 5 Excited-state Properties I will love the light for it shows me the way, yet I will endure the darkness for it shows me the stars. Og Mandino A common physical phenomena such as magnetism required the development of civilization to proceed whereas the much more elementary concept of light appeared before mankind−the first primitive experiments can be traced back to the taming of fire by man. However, it was first after the renaissance that mankind started to consider light as a scientific matter of importance. Dielectric functions and conductivity are the most important response functions in condensed matter physics because they determine the optical properties of materials, electrical conductivity, and a host of technological applications. In addition, optical spectra are perhaps the most widespread tools for studying the electronic excitations themselves. With the preceding chapters as a background we will now proceed to the study of excited-state properties. 5.1 Excitations in Density-Functional Theory Excitations in condensed matter are usually small perturbations on the entire system. Using perturbation techniques, one can calculate excitation spectra and the real and imaginary parts of the response function. Nevertheless, one needs to know the ground state, since the excitations are perturbations on the ground state. Spectroscopic techniques such as photoemission spectroscopy are very common in the study of ground-state properties of materials. In photoemission spectroscopy, high-energy photons are bombarded on a system, producing a current of photoelectrons. The energy of these photoelectrons is a measure of their binding energy in the material. The higher the energy of photons or electrons, the more is the perturbation of the ground-state electronic structure. CHAPTER 5. EXCITED-STATE PROPERTIES In general, if the perturbation due to the experimental procedure is kept to a minimum, then the results will more closely reflect the ground state of the system. This criterion is satisfied in optical spectroscopy since the energy involved in the excitations is a couple of tens of eV and both the initial and final states belong to the valence bands. However, the resulting spectrum will have a complicated dependence on the dispersion, which makes interpretation difficult and very indirect. Using modern band-structure calculations, the problem of deconvoluting the optical spectra can be avoided. Instead, a calculated version of the optical spectrum for a system is derived, and if the agreement between experiment and theory is good, the origin of the peaks in the spectrum can be easily extracted from the parameters used to calculate the spectrum. Moreover, if several models of the ground-state electronic structure exist for a system, optical spectra can be calculated for these different models, and compared with the experimental spectrum. Thus a particular model can be validated. The calculation of DOS, band structures, photo-emission spectra and optical properties using DFT relies on the identification of the KS eigenvalues (eigenfunctions) with the true eigenvalues (eigenfunctions). DFT is often quoted to be a ground-state theory and it is usually believed that it has little bearing on excited states. However, this is not correct. A basic consequence of the Hohenberg-Kohn theorems is that the ground-state density actually determines the Hamiltonian of the system. The reason is that the external potential (which is the only operator in the Hamiltonian that differs from system to system) is given by the ground-state density. Since the Hamiltonian completely characterizes all states of the system, the ground state density determines not only ground-state but also the excited states [41]. In spite of the above fact, it may be argued that the KS eigenvalues and eigenfunctions are just artificial constructions resulting from the one-particle approximation. However, the KS orbital eigen values are not completely devoid of physical meaning [41]. Their difference is a well defined approximation to the excitation energies in the electron-electron interaction of zeroth order. 5.2 Definition of the Conductivity Tensor The phenomenological formulation of Maxwell’s equations in the presence of polarizable or conducting media can be cast in terms of the complex frequency-dependent dielectric function (ω) or conductivity σ(ω). When a system is subjected to a time-dependent electric field E(r,t), an induced charge current J(r,t) will appear as a response. In the linear approximation, the relationship becomes: t 3 dtσ(r, r , t, t )E(r , t ) (5.1) J(r, t) = d r −∞ where the kernel σ (r,r ,t,t ) is called the conductivity. In an isotropic material, J and E are parallel, and the conductivity can be described by a scalar. However, in a real crystal, the two fields will not be parallel, and in this case the conductivity is a tensor of rank two. 60 5.2. DEFINITION OF THE CONDUCTIVITY TENSOR If the properties of the crystal do not change with time, the conductivity will only depend on the time difference t−t . Furthermore, when translational symmetry is present, the spatial dependence will follow r − r , viz. described by a vector in the Wigner-Seitz cell. We can then Fourier transform over both space and time, which gives the much simpler relationship J(ω, q) = σ(ω, q)E(ω, q) (5.2) where ω corresponds to the frequency of a plane electromagnetic wave and q is a crystal wave vector in the first Brillouin zone, and corresponds to the momentum transfer in the excitation of the electrons by the photon, i.e., it is the photon momentum. In the optical energy range, q is very small compared to the momentum of the electrons, and is therefore often neglected. For finite q, one can divide the conductivity into a transversal and a longitudinal part, depending on the relative orientation of q and E [42]. Here, we are only interested in the limit q→0, where this distinction disappears. An equivalent relationship can be obtained for the unitless dielectric function (ω,q), the relation between this entity and the conductivity being σij (ω, q) = iω [δαβ − αβ (ω, q)] 4π (5.3) in electrostatic units, which is the unit system used in this chapter, and i, j are Cartesian coordinate indices. A discussion of optical properties can be done using either of these tensors. 5.2.1 Symmetry considerations The optical conductivity tensor is symmetric in the absence of a magnetic field. In a coordinate system based on the principal axes, the conductivity tensor becomes diagonal. For crystals with high symmetry, some components will be equal. For example, cubic crystals have equal diagonal elements, and the tensor will have the same properties as a scalar. The presence of a magnetic field will change the symmetry properties of the conductivity tensor. It is no longer symmetric. However, the number of independent terms does not increase. As an explicit example, we take the case with the magnetic moment along the z direction, and with at least three-fold rotation symmetry around the z axis. The form of the optical conductivity tensor then becomes: ⎞ ⎛ σxx σxy 0 (5.4) σ = ⎝ −σxy σxx 0 ⎠ 0 0 σzz The Kubo formula [43] provides the link between band structure calculations and the macroscopic theory outlined above. A detailed derivation is given in Ref. [44]. The Kubo formula for the conductivity at finite temperature is, 0 N e2 1 δab + dt[ja (q, 0), jb (−q, t)]0 e−iωt , (5.5) σab (q, ω) = − imω h̄ω −∞ 61 CHAPTER 5. EXCITED-STATE PROPERTIES where a and b are Cartesian coordinate indices, N is the number of electrons per unit volume, and jb (q,t) is a component of the electron current operator in the interaction representation. The symbol 0 around the commutator indicates a thermodynamic average with the equilibrium distribution function. This just means that we take the sum over all states |n, weighted with the occupation. Expanding the commutator, putting in the identity operator n |n n | between the two current operators, transforming j β (−q,t) to Schrödinger representation, and taking the limit of direct transitions, q→0 gives, 1 1 −βn 0 e dt(n|jα |n n |jβ |neiωn n t −n|jβ |n n |jα |ne−iωn n t )(e−iωt −1), σαβ (ω) = h̄ω Z −∞ nn (5.6) where h̄ωn n = n − n and nn e−βn is the partition function (β = 1/kB T and n is the energy of state |n). The integral over time can be calculated by introducing a positive damping factor which results in Lorentzian broadening of the states, simulating finite lifetimes. The absorbed photon therefore may have slightly higher or smaller energy than the energy difference between the states. The states |n and |n are many-body states. In the one-particle approximation, the only matrix elements contributing are those between an occupied Bloch state and one that is unoccupied. This means that the sum over many-body states can be replaced by the sum over one-particle states. Thus, |n can be thought of as denoting occupied one-particle states, whereas |n refers unoccupied one-particle states. The relation between the current and momentum operators, j = (e/m)p, and the zero temperature limit are taken into account. Furthermore, our wavefunctions are Bloch functions and thus depend not only on r but also on crystal momentum k. Therefore we have to integrate also over reciprocal space. The real, (or absorptive) part of the conductivity (1) denoted σαβ (ω), can thus be written as, (1) σab (ω) = V e2 d3 kkn|pa |kn kn |pb |kn × fkn(1 − fkn )δ(kn − kn − h̄ω). (5.7) 8π 2 h̄m2 ω nn where kn is the energy eigenvalue corresponding to eigenfunction |kn , and V /(8π 2 ) is the normalization constant for the integral over reciprocal space, which is performed using the tetrahedron method. In this formula, the division between occupied and unoccupied states is taken care of through their Fermi distribution functions f kn and fkn . We now have a formula for the absorptive part of the conductivity. In order to calculate reflectivity of Kerr spectra, we also need the imaginary (or dispersive) part. This part of (2) the conductivity denoted as σ ab (ω) can be calculated from the absorptive part using the Kramers-Kronig (KK) transformation since the absorptive and dispersive components of the conductivity are interdependent through the KK relations. These relations are based on the assumption that no current can respond to the electric field before the electric field has arrived, i.e., cause precedes the effect (also known as causality theorem). 62 5.2. DEFINITION OF THE CONDUCTIVITY TENSOR 5.2.2 Broadening In order to compare the calculated optical spectra with experimental data, it is often necessary to perform broadening, thus simulating the physical mechanisms, which give the smearing of the experimental spectra. The most important effect is probably the finite lifetime of the excited states. Other contributions include temperature effects, indirect transitions, and experimental resolution. The effect of finite lifetimes can be simulated by convoluting the absorptive conductivity spectrum obtained by Eq. 5.7 with a Lorentzian. The lifetimes are state dependent, since high-lying excited-energy states are found to be more unstable and to have shorter lifetimes than the lower-lying ones. Thus, in principle the width of the Lorentizian should be function of the states involved in the excitation. Smearing due to temperature effects, indirect transitions and experimental resolution may all together be simulated by convoluting the spectrum with a Gaussian. Naturally, resolution broadening should be performed on the final spectrum, e.g., the reflectivity. In the other cases, it is always safe to perform the broadening on the absorptive spectrum. If the broadening is performed with a constant width, it can also be performed on the dispersive spectrum separately. 5.2.3 Indirect interband and intraband contributions The expression for the conductivity in Eq. 5.7, only takes direct interband transitions into account. In addition to these transitions, there are indirect interband and intraband transitions. Indirect transitions result from momentum conserving interaction between the electronic excitation and lattice imperfections, notably phonons. The effect of the indirect interband transitions is only a slight broadening of the structures in the optical spectra. If the material has an indirect energy gap, the optical gap will obtain a “foot". The calculated optical dielectric tensor for the case of ferrimagnetic YBaMn 2 O5 (Fig. 5.1)displays such a “foot" from 0 to 1 eV due to an indirect band gap. Intraband transitions can not take place in a material with a band gap (insulator or semiconductor) since no bands are partially occupied. The opposite is true for metals where low-energy intraband transitions constitute an important part of the total response for the diagonal components of the conductivity tensor. They are usually modeled with the Drude formula (which is based on the free-electron model): σD (ω) = ωP2 4π(γD − iω) (5.8) where γD is the inverse relaxation time and ωP is the (unscreened) plasma frequency. The plasma frequency can be calculated by integrating over the Fermi surface and can thus be predicted from band-structure calculations. In the free-electron model, the relation between the plasma frequency and the number of electrons per unit volume N is given by ωP2 = 4πN e2 , m 63 (5.9) CHAPTER 5. EXCITED-STATE PROPERTIES 15 E || a E || c ε1(ω) 10 5 0 E || a 8 ε2(ω) E || c 4 0 2 4 6 8 10 12 14 Photon Energy (eV) 16 18 20 Figure 5.1: Imaginary (upper panel) and real (lower panel) part of the optical dielectric tensor for ferrimagnetic YBaMn2 O5 along the crystallographic a and c directions. which can be used as a definition of the effective number of electrons N ef f per unit volume. The other Drude parameter, γ D , may change from sample to sample of a given material, since it depends on the amount of impurities and dislocations. 5.3 Extracts of theory of optics Experimental optical results are reported in the form of reflectivity spectra, energy loss, absorption, refractive indices, and changes in the direction of polarization upon reflection or transmittance. In order to compare calculated and measured spectra, the relations between the conductivity tensor and these quantities must be known. It is useful to start from the expression for a plane wave E(r, t) = E0 ei(ωt+bf kṙ) . (5.10) In the following formulae, the Cartesian coordinate subscripts and the functional dependence on ω have been suppressed. 64 5.3. EXTRACTS OF THEORY OF OPTICS 5.3.1 Index of refraction When a plane wave is propagating through a material, the velocity of propagation is different from that of vacuum, and the amplitude may be attenuated. These effects can be described by replacing the wave vector k in the plane wave by Nk. The function N is the (complex) index of refraction, written as N = n + ik, where n is called the (real) index of refraction and k the extinction coefficient. The relation between N and the dielectric function is simply (5.11) N2 = which follows from Maxwell’s equations. Using the relation Eq. 5.3, N can be calculated from the conductivity. 5.3.2 Reflectivity The reflectivity is the ratio between the incident and reflected light intensities. Since the intensity is proportional to the square of the wave amplitude, this can be written as R=r∗r (5.12) where r is called the reflection coefficient and is the complex ratio between the incident and the reflected electric field of the plane wave. For a normal incidence, the reflection coefficient is given by [45] N−1 (5.13) r= N+1 and the reflectivity becomes (N − 1) 2 R= . (N + 1) (5.14) 5.3.3 Absorption coefficient The absorption coefficient α is defined as α=− 1 dI I dr (5.15) where I is the intensity of the plane wave at a distance r inside the material. By differentiation of I expressed using the plane wave, one finds that α is proportional to the imaginary part of the refractive index times the frequency: α= 2ωk . c 65 (5.16) CHAPTER 5. EXCITED-STATE PROPERTIES 5.3.4 Energy loss When a beam of mono-energetic electrons impinges on a solid, excitations in the solid, (e.g., plasmon excitations or interband transitions) result in energy losses of the electron beam. In this case, the electric field causing the response is in the direction of propagation of the beam, and not perpendicular to it, as is the case for photons. From dielectric theory one can show that the energy loss of the electron beam is proportional to the energy loss function L, which is defined as 1 (5.17) L = −Im . 5.4 A note on spin-orbit coupling The spin-orbit coupling is important for heavier elements and is required in the calculation of the magneto-optical effects. The spin-orbit coupling term is written as, ξ(r)l · s (5.18) where ξ is the spin-orbit coupling strength ξ(r) = 1 1 dV . 2m2 c2 r dr (5.19) Normally, spin-orbit interaction is included in the calculational scheme by incorporating this term in the calculation of the Hamiltonian matrix elements inside the muffin-tin spheres. The operator l · s = lx sx + ly sy + lz sz can be rewritten using ladder operators as s ± = sx ± isy and l± = lx ± ily . The spin-ladder operators act on the spin components, for example s ± will turn spin down into spin up. Similarly, the orbital-ladder operator acts on the spherical harmonics, increasing or decreasing the magnetic quantum number m by one. Therefore, direct inclusion of spin-orbit coupling doubles the size of the matrix to be diagonalized since spin up and spin down are mixed. In the LMTO methods relatively little time is consumed for matrix diagonalization. However, in the case of LAPW method, the matrices are large and diagonalisation of them requires substantial computational efforts. Therefore, spin-orbit is usually included as a second variational step, which is workable as long as the coupling is not too large. 5.5 Calculation of Magneto-Optical Properties Plane-polarized light, when reflected from a metal surface or transmitted through a thin film with non-zero magnetization, will become elliptically polarized, with its major axis slightly rotated with respect to the original direction. The effect due to transmission is called the MO Faraday effect, and that due to reflection is known as the MO Kerr effect (MOKE) [46, 47]. The Kerr effect exists in several different geometries. Of these, the polar Kerr effect (for 66 5.5. CALCULATION OF MAGNETO-OPTICAL PROPERTIES which the direction of the macroscopic magnetization of the ferromagnetic material and the propagation direction of the linearly polarized incident light-beam are perpendicular to the plane of the surface) is by far the largest. Therefore the polar-Kerr geometry is the most interesting in connection with technological applications. Hence, we performed our theoretical investigations for the polar Kerr effect only. With the magnetic moment in the [001] direction of say, a hexagonal crystal, the optical conductivity tensor will take the form of Eq. 5.4. Consider a plane-polarized light beam traveling in the z direction which is parallel to the magnetization direction M. This light beam can be resolved into two circularly polarized beams with the spinning direction of the corresponding electric field parallel and antiparallel to M. We use the sign convention in which right-circular polarized (RCP) light has its electric field vector E rotating in a clockwise sense at a given point in space. The signs of Faraday rotation θF and Kerr rotation θK are positive for a clockwise rotation of the axes of the polarization ellipse, as viewed by an observer who looks in +z direction when the incoming linearly polarized light from a source is traveling along the +z direction. For the polar geometry, the Kerr rotation and ellipticity are related to the optical conductivity through the following relation, (1 + n+ )(1 − n− ) 1 + tan(ηK ) 2iθK e , = 1 − tan(ηK ) (1 − n+ )(1 + n− ) (5.20) where n2± are eigenvalues of the dielectric tensor corresponding to Eq. 5.4. In terms of conductivities, they are n2± = 1 + 4πi (σxx ± iσxy ). ω (5.21) For small Kerr angles, Eq. 5.20 can be simplified [48] to θK + iηK = −σxy . σxx 1 + 4πi σ xx ω (5.22) The magnetic circular birefringence, also called the Faraday rotation θF , describes the rotation of the polarized plane of linearly polarized light on transmission through matter magnetized in the direction of the light propagation. Similarly, the Faraday ellipticity η F , which is also known as the magnetic circular dichroism, is proportional to the difference of the absorption for right- and left-handed circularly polarized light [47]. Thus, these quantities are simply given [49] by: θF + iηF = ωd (n+ − n− ) , 2c (5.23) where c is the velocity of light in vacuum, and d is the thickness of the film material under investigation. 67 1 θK εK 1 θF εF 0 0 Faraday Rotation θF and Ellipticity εF (deg.) Polar Kerr Rotation θK and Ellipticity εK (deg.) CHAPTER 5. EXCITED-STATE PROPERTIES −1 Ba2FeMoO6 −1 −2 0.5 2 0 −0.5 −2 Ba2FeWO6 −1.5 −4 2 1 0 0 −2 Ba2FeReO6 −1 0 1 2 3 4 5 6 −4 1 2 3 4 5 6 Energy (eV) Figure 5.2: The calculated polar Kerr rotation (θ K ), Kerr ellipticity (K ), Faraday rotation (θF ), and Faraday ellipticity ( F ) spectra for Ba2 FeBO6 with B = Mo, W, and Re. We have performed extensive calculations on magneto-optical properties for A 2 FeBO6 (A = Ca, Sr, Ba; B = Mo, W, and Re) and found that most of the compounds in that series have very high Kerr and Faraday rotations at 0 K. Readers can observe the large magneto-optical effects (of the order of ∼1.5◦ Kerr and 2−4◦ Faraday rotation) for Ba2 FeBO6 (B = Mo, W, and Re) as exemplified in Fig. 5.3. It is worthwhile to recall here that Kerr rotation value of ∼2.5 ◦ has been observed for one of the Heusler alloys, PtMnSb [50]. However, we believe that our finding of large magneto-optical values may be the highest for any oxide material. As these compounds have magnetic transition temperature (T C ) around 400 K and also half-metallic electronic structure, we anticipate that they may have important technological applications (Publication IVX). 5.5.1 Magneto-optical figure-of-merit In order to extract the written information in a MO medium easily, and to make the signal-to-noise ratio as high as possible, the MO figure of merit (FOM) [51] should be large. FOM is defined [52] as, F OM ≈ 2 + 2 ), R(θK K (5.24) where R is reflectivity and θK and K are as defined earlier. FOM is often used to characterize and evaluate the performance of a MO medium fabricated by different manufacturers. However, FOM depends on the structure on to which the magnetic material is embedded, a 68 5.6. CALCULATION OF XANES Ca2FeMoO6 Ca2FeWO6 Ca2FeReO6 0.75 0.25 Sr2FeMoO6 Sr2FeWO6 Sr2FeReO6 Figure of Merit (deg.) 1.5 0.5 Ba2FeMoO6 Ba2FeWO6 Ba2FeReO6 0.75 0.25 0 1 2 3 4 5 Energy (eV) Figure 5.3: Magneto-optical figure-of-merit for A 2 FeBO6 with B = Mo, W, and Re. large FOM value is one of the many indications for applicability of MO materials. The FOM values calculated for the double perovskites A 2 FeBO6 (A = Ca, Sr, Ba; B = Mo, Re, and W) compounds are comparable with that for the well-known MO material PtMnSb, and we believe that these large FOM values can motivate more experimental MO studies on these compounds. 5.6 Calculation of XANES We have computed x-ray absorption spectra in this project for systems like YBaMn 2 O5 and CaRuO3 , within the dipole approximation from the FPLAPW (Wien2K) partial DOS along the lines described by Neckel et al. [53] The intensity I(ω) = E − E c arising from transitions from initial VB states (energy E and and angular momentum ) to a final core state (Ec , ) is given by: Iτ n l (ω) = W Mτ2 (, n , E)Dτ (E)δ(E − Encore − h̄ω) ω3 69 (5.25) CHAPTER 5. EXCITED-STATE PROPERTIES where the matrix elements are given by Rτ Mτ2 (, n , E) = 0 Pτ (r, E)rPn prime (r)dr Rτ 2 τ 0 P (r, E) dr 2 n and represent principal and angular momentum quantum numbers for the core states, Dτ (E) is the partial DOS of atom τ with angular momentum ; Pτ and Rτ being the radial wave function and atomic sphere radius of atom τ . The transition coefficient W can be calculated analytically according to the equation, W = +1 δ, −1 + δ, +1 2 + 1 2 − 1 For absorption spectra Dτ (E > EF ) = 0. To account for instrumental resolution and lifetime broadening of core and valence states we have broadened the calculated spectra using a Lorentzian function with FWHM of 1 eV. 70 CHAPTER 6 Magnetism and Spin Ordering Imagination is more important than knowledge. Albert Einstein 6.1 Magnetic classes Inorganic solids that exhibit magnetic effects are characterized by having unpaired electrons. It has long been known that such materials acquire a magnetic moment M when exposed to a magnetic field H. The amount of induced magnetization of the material in an applied field is given by, M = χH (6.1) (in general, M = χH) where χ is termed magnetic susceptibility. For a large special class of materials the induced magnetic moment is oppositely aligned to the applied magnetic field viz. χ < 0. This behavior is called diamagnetism which is omnipresent in every material including the magnetic materials which are discussed below. Compared with the other forms of magnetism the effect of diamagnetism is small. The most important magnetic materials have non-zero atomic magnetic moments, i.e., each atom carries a magnetic moment. In large classes of materials these moments will be uncorrelated (under certain conditions: notably in the absence of an external magnetic field), and point randomly in arbitrary directions resulting in a zero net moment (Fig. 6.1a). M= Mi = 0 (random; P state) (6.2) where Mi is the magnetic moment of atom i. When a magnetic field of a certain magnitude is applied, these atomic moments will be aligned by the applied field. The total moment behaves according to the above equation with χ > 0 (in general with M and H as vectors and χ as a tensor) and the magnetic susceptibility χ becomes a temperature function. Such CHAPTER 6. MAGNETISM AND SPIN ORDERING (a) (b) (c) (e) (d) Figure 6.1: Schematic illustration of possible simple arrangements of atomic magnetic moments in (a) paramagnetic, (b) ferromagnetic, (c) collinear antiferromagnetic, (d) canted antiferromagnetic, and (e) ferrimagnetic order. More exotic forms of co-operative magnetism like helimagnetism etc. are not included since such arrangements are not found among the phases included in this study. materials are called paramagnetic materials. While the applied field favors alignment of local moments in its direction, the thermal disordering effect opposes the alignment. Another class of materials, known as ferromagnetic materials, do not need an external magnetic field to get magnetized, they exhibit spontaneous magnetization [Fig. 6.1(b)]. M= N Mi = N · Mi (F state) (6.3) i Among the pure elements Fe, Co, Ni, and some rare-earths provide examples of ferromagnetic materials. At sufficiently high temperatures ferromagnetic materials transform into a paramagnetic state and in the absence of a magnetic field their atomic magnetic moments point in arbitrary directions, cancelling each other and resulting in zero net magnetization. At the temperatures concerned the thermal fluctuations of the moments are so high that the aligning tendency of the atomic moments is surmounted. When the temperature is reduced, the interaction between oriented atomic moments start to compete with the thermal disorder effects. When the temperature is further reduced to a value known as Curie temperature TC , a transition to the ferromagnetic state occurs. Below T C the interaction between non-zero atomic moments overcomes the thermal fluctuations, resulting in a net spontaneous magnetic moment even without the application of an external field. The magnetic susceptibility in the paramagnetic state is given by, χ= C , f or T > Θ ≈ TC T −Θ 72 (6.4) 6.1. MAGNETIC CLASSES where C is named as the Curie constant and Θ the Weiss constant. The above equation is named as the Curie-Weiss law. Simple antiferromagnetic systems comprise oppositely aligned atomic magnetic moments, the vectorial sum of which becoming zero by symmetry, below an ordering temperature known as the Néel temperature (T N ). M= N Mi = 0 (cancelling; AF state) (6.5) i Above TN the paramagnetism rules and the temperature variation of the magnetic susceptibility is also in this case described by equation (2). The Weiss constant is related to T N by TN ≈ −Θ. A considerable amount of efforts has been made over the years to understand the origin of magnetism using both classical physics and quantum mechanics. It was eventually Dirac’s relativistic quantum theory that explained the spin quantum state of electrons. The spin magnetic moment can be regarded as an extra degree of freedom for the electron − it can be either in a “spin up” or in a “spin down” configuration. The concept of spin falls out naturally from the solutions of the eigenvalue problem and is intimately connected with relativity. Electrons are treated as waves in quantum mechanics and the overlap of such waves is reflected as an interaction between the spins of different electrons. If this so-called “exchange interaction” is strong enough, the material will experience co-operative ordering of the spin moments. A common way to handle such exchange interaction is to use the socalled “mean field approximation” In this approach one spin is considered to be influenced by the exchange interaction from the mean field from all other spins. After manipulation, this initially fixed spin is released and treated so that it becomes on equal footing with the other spins. It should also be noted that the atomic moments comprise contributions from both the spin magnetic moment and the orbital magnetic moment. The latter moment originates from the orbiting of an electron (a charged species) around the positive nucleus (a source of the electric field). The ground state of a free atom or ion (like rare-earth 4f ions) with a perfect spherical symmetry has an orbital magnetic moment in accordance with Hund’s second rule. For a 3d-transition-metal atom the electric field from neighboring atoms (the crystal field effect) normally breaks the spherical symmetry conditions and the orbital moment becomes “quenched” and such an atom is said to obey the “spin-only” approximation. When the spin-orbit interaction energy is introduced as an additional perturbation on the system, the spin may, under certain conditions drag some orbital moment along with it [54]. If the sign of the interaction favors parallel orientation of the spin and orbital moments, then the total moment will become larger than the spin-only value. Thus the spin-orbit coupling removes parts of the quenching of the moments at the spin value and results in turn in a directional preference of the spin moment. 73 CHAPTER 6. MAGNETISM AND SPIN ORDERING A−AF G−AF C−AF Ferri Figure 6.2: Schematic diagram indicating possible different types of antiferromagnetic spin ordering in perovskite-like oxides. 6.2 Types of antiferromagnetic spin ordering Since one of the aims of the present thesis has been to study transition-metal oxides, performing calculations in the respective co-operative magnetic states has been mandatory. Therefore, we have conducted theoretical simulations for paramagnetic (P), ferromagnetic (F), and antiferromagnetic (AF) configurations of a given system. Sometimes, in addition to the experimentally found or suggested magnetic states, we also considered other possible magnetic orderings in order to obtain a broader platform for judgement of the magnetic arrangement. In perovskite-like oxides, the AF spin ordering can take different configurations according to the inter- and intraplane spin-couplings as described below. A-type AF: This configuration occurs when the interplane coupling is antiferromagnetic and the intraplane coupling within (001) is ferromagnetic, [Fig. 6.2(a)]. (For example, undoped LaMnO3 with orthorhombic structure has an A-AF arrangement). C-type AF: This configuration is opposite to A-type ordering, i.e., the interplane coupling is ferromagnetic and intraplane coupling is antiferromagnetic, forming a chain-like ordering [Fig. 6.2(b)]. (The orthorhombic LaCrO3 has and C-AF structure as its ground-state magnetic structure.) G-type AF: In this case, both inter- and intraplane couplings are AF [Fig. 6.2(c)]. [This kind of ordering is commonly seen in RBaMn2 O5 (R = Y and La; Publications I to V)]. 74 6.3. EXCHANGE INTERACTION The orthorhombic perovskite-oxide SrRuO 3 is found to be a ferromagnetic metal whereas the magnetic ground-state of CaRuO3 is shrouded under controversy. In order to find out the exact magnetic ground-state structure for CaRuO 3 , and to understand the reason for its distinction from SrRuO3 , we have considered all the above magnetic orderings for a series of Sr1−x Cax RuO3 (x = 0, 1/4, 1/2, 3/4, and 1). We arrived at a conclusion that CaRuO3 has a spin-glass-like behavior. The results are dealt with in Publications (XII and XIII). We have seen that based on these orderings, the electronic structure also undergoes noticeable changes. CE-type AF: In this case the magnetic cell is a quadrupled chemical unit cell with zig-zag arranged F chains of magnetic atoms that are AF coupled with nearest neighboring chains. In optimally doped perovskites (e.g., La 1−x Srx MnO3 , x = 1/2), the most common magnetic order is the CE-type AF order. However, as this type of ordering is computationally very demanding (really too complex to handle), we have not considered it in our calculations. Canted antiferromagnetic structure and non-collinear magnetic arrangements were not included in our calculations. Ferrimagnetic: In ferrimagnetic (Ferri) ordering [Fig. 6.2(d)], the situation is basically the same as in a corresponding AF arrangement, but the atoms bearing opposite magnetic moments occur in different quantities and/or their magnetic moments differ in size. As a consequence, the moments do not compensate to give a resulting zero total moment for an individual crystallite. The overall behavior of Ferri materials in a magnetic field is like that of F materials [55]. In the present thesis, one finds several examples of Ferri systems. In YBaMn 2 O5 (Publication I), the Ferri state results from differently-sized non-cancelling moments on two crystallographically different Mn sites (formally Mn3+ and Mn4+ ). In Sr2 FeMoO6 (Publication XIV), the oppositely arranged magnetic moments of Fe and Mo are of different size, again leading to Ferri state. In the case of one-dimensional Ca 3 Co2 O6 , a triangular network of Co-O chains are formed. The moments of Co are F aligned along the chains. For every two F-aligned chains there is one AF-aligned chain resulting in a Ferri state. 6.3 Exchange interaction If the magnetic species in a solid do not communicate with each other, Eq.(1) simplifies to Curies Law in which Θ = 0 K and co-operative magnetic ordering is prohibited. Magnetic exchange interaction in oxides does normally not involve communication via conduction electrons. In most oxide cases the direct exchange interaction between the moment-carrying transition-metal atoms is out of the question owing to the long metal-to-metal separations in the crystal structure. The only example of a phase with probable direct exchange interaction in this thesis is provided by Ca3 Co2 O6 (Publications X and XI). For the magnetic exchange 75 CHAPTER 6. MAGNETISM AND SPIN ORDERING 0 1 0 1 11 00 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 3+ 0 1 11 00 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 O Mn 2− 0 1 11 00 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 Mn4+ 4+ Mn 0 1 11 00 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 0 1 00 11 2− O Mn3+ Figure 6.3: Schematic illustration of double-exchange interaction between Mn4+ and Mn3+ via an intermediate O2− . information path in oxides one is accordingly left with indirect exchange interactions either of the double- or super-exchange types. 6.3.1 Double-exchange interaction In order to rationalize the spin-ordering phenomena and associated changes in electrical conductivity in transition-metal oxides, the concept of double-, and super-exchange interactions has been invoked. The most important interaction in magnetic materials is the double-exchange interaction [56, 57]. Transition-metal atoms arranged in a periodic array in a crystal lattice may be subjected to exchange interactions between the spins of unpaired electrons associated with the atoms concerned. For a transition-metal atom contained in a perovskite-type structure surrounded by six O atoms, the wave functions (orbitals) pointing toward the oxygen ions (d z 2 and dx2 −y2 , denoted as eg ) have higher energy than those pointing between them (dxy , dyz , and dzx , named t2g orbitals) [58]. When electrons occupy these orbitals, the ground state is determined by the semiempirical Hund’s rule. The spins of the eg electrons of a transition-metal atom are forced to be parallel to the localized t2g spins (by the usually strong) Hund’s coupling J H . When an eg electron hops between atoms, its spin wave function is coupled to the spin direction of the t 2g spins at the atom concerned. Therefore, the effective transfer integral (t ij ) is considered to be proportional to cos(Θij /2), (where Θij is the angle between the two spin directions). The transfer integral depends on the relative direction of the two spins: it takes a maximum value for parallel spins and zero value for antiparallel spins. Therefore, the kinetic energy gain of the electrons is maximized for parallel spin, which leads to the F interaction between the spins and efficient transfer of electrons between the atoms. This mechanism is called doubleexchange interaction. For example, for a system containing Mn3+ and Mn4+ intervened by 76 6.3. EXCHANGE INTERACTION 00 11 00 11 11 00 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 3+ Mn 00 11 11 00 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 00 11 O 2− 3+ Mn Figure 6.4: Schematic illustration of super-exchange interaction between two Mn3+ via O2+ . an O2− , there is simultaneous transfer of one electron between Mn 3+ and the neighboring O2− and from thereon to Mn4+ . The limiting configurations Mn3+ -O2− -Mn4+ and Mn4+ O2− -Mn3+ will be degenerate if the spins of the two d shells are parallel, and represents the lowest energy state of the system at low temperature. It should be emphasized that the F double-exchange interaction is characterized by short-range electron hopping between atoms, and this process can be terminated at any point in the lattice and accordingly preventing a three-dimensional conductivity. Double exchange always results in F configurations unlike super-exchange which involves virtual electron transfer and frequently leads to AF arrangements [59]. 6.3.2 Super-exchange interaction Super-exchange interaction is one of the processes by which coupling of magnetic moments promotes an AF state. For example, let us consider LaMnO 3 where Mn3+ carry four d electrons and O2− two p electrons. The half-filled eg orbital is oriented so as to point directly at adjacent oxygen atoms. The unpaired electron in the e g orbital of Mn3+ is able to couple magnetically with electrons in the p orbitals on O2− . This coupling may well involve the formation of an excited state in which the electron is transferred from the e g orbital to the oxygen p orbital. The p orbitals of O2− contain two electrons each, which are mutually coupled antiparallel. Hence, a chain coupling effect occurs which extends through the entire crystal structure (Fig. 6.4). The net effect of this is that neighboring Mn 3+ ion in LaMnO3 (along c direction), separated by intervening O2− , are coupled antiparallel [60]. The essential point in the super-exchange mechanism is that the spin moments of the transition-metal atoms on opposite sides of an oxygen atom interact with each other through the p orbital of the latter. The super-exchange interaction is expected to be the strongest for a bond angle 77 CHAPTER 6. MAGNETISM AND SPIN ORDERING of 180o . The difference between double- and super-exchange lies basically on the filling of intermediate oxygen p orbital, the valence-state of the transition-metal atoms involved, and the position of these atoms relative to one another. 78 CHAPTER 7 Charge and Orbital Ordering A profound truth is a truth whose opposite is also a profound truth. Niels Bohr 7.1 Mixed-valence transition-metal oxides Transition-metal oxides have been intensively studied in recent years in order to elucidate relationships between structure, bonding, and magnetic properties motivated both by intrinsic interest in the subject itself and also owing to the extraordinary technological potential of these materials. The transition-metal oxides are traditionally regarded as compounds 1 formed by oxygen anions with completely-filled valence shells and cations of transitionmetals with an incompletely-filled d shell. The situation becomes somewhat messy because the incomplete d shells do not represent universally stable configurations, and the cations tend to exist in various valence states depending on the actual constituents and external factors like temperature, pressure etc. It must be appreciated that the metal atoms are located in an environment consisting of oxygen anions and other cations, and thus subjected to the complex influence of the immediate crystal field and more long-range electrostatic forces as well as magnetic interactions. The combination of all such effects determines the degree of the localization of the outer electrons, viz. their pertinence to definite atoms. Therefore it is appropriate to distinguish between materials exhibiting a high degree of localization (as found in magnetic oxides where ions that possess various valences can be present simultaneously in the crystal lattice) and those with itinerant charge carriers (as in superconducting oxides [61]). Compounds with mixed-valence (MV) transition-metal ions have been widely studied 1 In this chapter, covalent interactions are neglected in a way that the presentation uses a purely ionic language. CHAPTER 7. CHARGE AND ORBITAL ORDERING for their interesting optical, electrical, and magnetic properties. Robin and Day have classified [62] mixed-valence compounds into three categories: (i) Class-I MV characterized by distinctly different co-ordination environments for constituents in different valence states. Such phases contain localized electrons and exhibit insulating/semiconducting behavior. (ii) Class-II MV are also characterized by different environments for the constituents in differing valence states, but the structural surroundings are sufficiently similar to allow electron transfer between some or all constituents with only a small input of energy. (iii) ClassIII MV exhibits delocalization of the valence electrons so that all of the MV atoms obtain the same chemical environment and the same valence state. Of particular interest are compounds that transform from either class-III or class-II MV to class-I MV upon cooling. This type of transition, triggered by electron localization, often leads to a phenomenon known as charge ordering. 7.1.1 Determination of valence states The charge ordering phenomenon which is elaborated on this thesis requires participation of mixed-valence transition-metal ions. For inorganic materials, valence or oxidation states of the constituents are commonly assigned on the basis of an ionic model, viz. electroneutrality is attained as if the compound under consideration is an ionic insulator. For example, in an ABO3 perovskite oxide like LaMnO3 , the starting point is the assumption that O acquires a completely filled valence shell (O2− ), La should be La3+ , and Mn should then be Mn3+ . However, as we have seen the bonding in our materials have mixed ionic and covalent character. Hence the assignment of valence states to transition metal atoms may be non-trivial. Over the years there has been quite a few empirical rules advanced for ascribing valence to binary, ternary etc. compounds like the Pauling rules, Hume-Rothery (8−N) rule etc. However, for compounds comprising of heavy elements, and in particular transitionmetals, the participation of electrons in magnetism makes the situation complicated. The valence of any element is determined by the involvement of the outer-most (valence) shell electrons in bonding and magnetism. In order to determine the most stable spin and valence configurations, the semi-empirical Hund rules are used: (i) The individual electron spins si combine to give the maximum value of the spin quantum number S in accordance with the Pauli principle. (ii) The orbital vectors li combine to give the maximum value of L in conformity with the Pauli principle. (iii) The resultant L and S combine to form J, the value of which is to be taken as J = L − S if the shell is less than half occupied, and J = L + S if the shell is more than half occupied. The measured magnetic moments at the transition metal sites in a given structure may be 80 7.2. INFLUENCE OF STRUCTURE ON ORDERING PHENOMENA viewed in relation to these rules. Even though measurement of magnetic moments and use of concepts like bond-valence sums can provide indications of the presence of mixedvalence states in a compound, such empirical facts do not allow firm conclusions about valence states. 7.1.2 Effects of crystal-field In addition to exchange interactions, crystal-field effects play an important role in determining the splitting of the d levels, and consequently in the choice between different valence states for transition-metal constituents. In free atomic states, every 3d electronic state has the same energy (viz. the energy levels are degenerate). When a transition-metal atom is surrounded by, say, oxygen ligands in tetrahedral, octahedral etc. configurations, the surroundings anions give rise to a strong electric field that splits the d levels into two groups, triply degenerate t 2g (dxy , dyz , and dxz with spatial distributions along xy, yz, and xz) and doubly-degenerate e g levels (dx2 −y2 and dz 2 orbitals with spatial distribution along the coordinate axes). The splitting of the d levels varies with respect to the magnitude of the surrounding crystal field as qualitatively illustrated in Fig. 7.1. Note that the population of the thus split d levels also has a deciding effect on the spin states of the atom concerned, referred to as low-spin, intermediate-spin, and high-spin states in the ionic terminology. In our efforts to determine valence states for transition-metal constituents in the studied systems, we make use of theoretically calculated magnetic moments as well as site- and orbital-projected DOS. For example, in our calculation on Ca3 Co2 O6 which has Co in octahedral and trigonal prismatic environments, we first arrived at the conclusion that the Co atoms exist in Co2+ and Co4+ states (Publication X). We are pleased to note that our findings stimulated many experimental and theoretical further studies on this compound. As more or less anticipated many of these reports rejected our proposal of a different oxidation state for the Co species and favored instead a common Co 3+ state in low-spin and high-spin configurations. However, using various analytical tools (Publication XI) we have later found that the problem is not so simple, but most of the controversy seem to originate from use of the ionic terminology on a compound which exhibits an appreciable covalent contribution to the Co-O bonding. 7.2 Influence of structure on ordering phenomena 2 Within the oxide family, perovskite-type materials (with general formula ABO3 ) are among the most exotic, and exhibit a wide spectrum of physical properties such as superconductivity, colossal magnetoresistance, various magnetic ordering features, ferroelectricity, thermoelectric properties etc., just to name a few. 2 Although many of the oxide materials dealt in this thesis work do not directly belong the perovskite family, a discussion on the structural features of perovskites are made in order to illustrate various ordering phenomena. 81 CHAPTER 7. CHARGE AND ORBITAL ORDERING dx2−y2 dxz dxy dz2 dyz d d dx2−y 2 dz 2 dxy dxz (a) dyz (b) dx2 y 2 − dx z dyz dz2 d d dx y dx 2− y 2 dxy dx z dz 2 dyz (d) (c) Figure 7.1: Pictorial illustration of the splitting of the d levels in (a) tetrahedral, (b) octahedral, (c) square-pyramidal, and (d) trigonal-prismatic crystal fields of idealized symmetry. No significance is to be attached to the separation between the d levels, neither within each part of the illustration nor between the different parts. Magnetoresistance (MR) is the relative change in the electrical resistance of a material produced on the application of a magnetic field. The ratio M R [|Δρ|/ρ(0) = |ρ(H) − ρ(0)|/ρ(0) where ρ(H) and ρ(0) is the resistance at a given temperature in the presence and absence of a magnetic field (H), respectively] can be negative or positive. Large magnetoresistance, [referred to as colossal magnetoresistance (CMR)] has attracted wide attention in particular for perovskite oxides. CMR can dramatically alter the electrical resistance and related properties of a material [63] revealing some remarkable features with regard to charge 82 7.2. INFLUENCE OF STRUCTURE ON ORDERING PHENOMENA and spin dynamics in addition to opening up new avenues for research. The potential industrial application has apparently accelerated the research activity, and as a result deepened our comprehension of the field. The structure of perovskite oxides is highly compact and sensitive to the size of the cationic constituents. Consequently, efforts to go beyond the tolerance limits for the geometrical requirements, challenge the structural stability and/or cause structural distortions. The minimum Gibbs energy decisive for the stability of a phase with a certain structure is given by the relationship: G = EC + Ecf + Eex + P V − T S (7.1) where EC is the Coulomb energy, Ecf the crystal-field stabilization energy, Eex the exchange energy, P V the energy associated with volume change, and T S the entropy contribution. The energy content in these terms reflect the interactions between the constituents as determined by structures, valence, electronic configuration, and atomic size etc. Note that details of the structural arrangement (like the oxygen environment) may have a considerable impact on the interactions concerned. Often there is an interplay between the various contributions and this results in, among other things, preference of certain constituents for certain sites and formation of an ordered state which in general leads to the lowering of the structural symmetry. 7.2.1 Effects of Jahn-Teller distortion One of the most-prominent structural distortion occurring in perovskite-like oxides is the co-operative Jahn-Teller distortion. The Jahn-Teller theorem [64] states that a non-linear system in an electronically degenerate state must undergo a distortion in order to remove the degeneracy, thereby lowering both the symmetry and the energy of the system. In an extended solid, where the polyhedra are linked to form a three-dimensional-bond network, the Jahn-Teller distortion that occurs at each polyhedron is felt also by the neighboring polyhedra. Consequently, the direction and size of the distortion must be co-operative throughout the crystal, an effect known as co-operative Jahn-Teller distortion (CJTD). This diffusionless CJTD process, in fact leads to a lowering of the total symmetry of the crystal. The resulting equilibrium can be regarded as a compromise between the increase in elastic and decrease in electronic energy consequent on the distortion (since the character and extent of the distortion is strongly influenced by the structural matrix as well as the constituents). In a transition-metal oxide, where each orbital of the transition-metal constituent has different anisotropy, the displacements of the surrounding O atoms are intimately coupled to the configuration of the d orbitals. For example, when the two apical O atoms in an octahedron move toward the central atom, the d z 2 orbital is shifted to higher energies than the dx2 −y2 orbital thus lifting the degeneracy of these orbitals. 83 CHAPTER 7. CHARGE AND ORBITAL ORDERING 7.3 Orbital Ordering Orbital ordering (OO) among the transition-metal oxides is concerned with the preferential occupation of electrons in specific d orbitals. The interaction of the orbital degrees of freedom among themselves and their interaction with electron spins or lattice, can give rise to long-range orbital-ordered states. Together with the charge and spin degrees of freedom they determine all the rich variety of the properties of transition-metal oxides. The orbital effects play a very important role in the physics of manganites, and also in many other transition-metal oxides. For example in an undoped rare-earth manganite, only Mn 3+ are present at the octahedral sites and the Jahn-Teller effect determines the arrangement of the dz 2 orbital subsequently leading to the orbital ordering. The orbital ordering gives rise to the anisotropy of the electron-transfer interaction. This favors or disfavors the double-exchange interaction and the super-exchange (ferromagnetic or antiferromagnetic) interaction in an orbital-direction-dependent manner and hence gives a complex spin-orbital-coupled state. According to the well known Goodenough-KanamoriAnderson rules [65] the magnitude and even the sign of the magnetic exchange depend on the type of orbitals involved and the filling of these orbitals. If orbitals are half-filled (occupied by one electron) and directed to each other, we will have a strong AF coupling. On the other hand, if these orbitals are directed away from each other (mutually orthogonal) we would have a F interaction. The orbital degree of freedom is thought to play important roles, not only in the prominent case of CMR manganese oxides but also in the anisotropic electronic and magnetic properties of a great many transition-metal oxides. Even though a lot of attention has been paid to manganese oxides, it should be noted that the orbital physics is universal in transition-metal oxides. 7.3.1 An example−LaMnO 3 Undoped LaMnO3 is well known to exhibit orbital ordering and a concomitant lattice distortion. LaMnO3 in the perovskite-like structure contains the Jahn-Teller Mn 3+ ions which are known to induce a rather strong local distortion. The e g orbitals of the Mn3+ ions are ordered in such a way that at the neighboring Mn sites the d z 2 orbitals are ordered alternatively along the x and y directions. The transfer integral between the two neighboring Mn atoms in the crystal lattice is determined by the overlaps of the d orbitals with the p orbital of the O atom between them. The overlap between the d 3x2 −r2 and pz orbitals is zero because of their different orientation with respect to the xy plane. Therefore, the electron in the d3x2 −r2 orbital cannot hop along the z axis and the individual MnO6 octahedra are alternatingly elongated along x and y directions. Owing to this OO, anisotropic super-exchange interaction results, viz. undoped LaMnO 3 has an A-type AF ordering, the spins in one xy layer exhibiting F order, and are antiparallel to the spins in the next xy layer. 84 7.4. CHARGE ORDERING b c a Figure 7.2: Orbital ordering in orthorhombic LaMnO3 . In order to elucidate the antiferro-type orbital order the dz2 orbitals are shown in blue and red colors. Note that the MnO6 octahedra are elongated along the lobes of the dz2 orbital. 7.4 Charge ordering Charge ordering (CO) is a phenomenon observed in solids wherein certain electrons defacto become localized as a result of ordering of cations of differing charges on specific lattice sites [66], thus often rendering the material insulating. CO has been known for many years in Fe3 O4 , the transition from the CO state to the charge-disordered state in Fe 3 O4 at 120 K (identified by Verwey [67] as early as 1939) is associated with a resistivity anomaly. In a perovskite manganite, when the trivalent cation is substituted by a divalent cation, there is variation in the amount of Mn3+ to Mn4+ ratio. When the ratio is 1:1 the OO occurs simultaneously with a long range ordering of Mn 3+ and Mn4+ mediated by Coulomb interaction. Such a type of ordering can strongly modify the crystal structure and accordingly also the magnetic interactions. Using the perovskite-like R 1−x Ax MnO3 phase as an example two correlation effects must be distinguished. First the ferromagnetic double exchange characterized by shortrange electron fluctuation mediated by dynamic occupancy of the e g orbitals. Second the structural transition driven by the orbit-lattice interaction of Mn3+ and controlled by the frequency of the electron hopping between Mn 3+ and Mn4+ which becomes frozen in at a sufficiently low temperature. These correlation effects compete with each other and one can easily imagine that the prevailing character will depend on the geometrical arrangement of the Mn-to-O-to-Mn bonds (viz. be strongly influenced by distortion from the ideal perovskite structure). With structural deformations follow lowering of the transfer integral for the eg electrons thus causing a weakening of the ferromagnetic interactions and a strong 85 CHAPTER 7. CHARGE AND ORBITAL ORDERING tendency to charge localization, viz. a preference for charge ordering. The phases with the R 0.5 A0.5 MnO3 composition is of particular interest because of the frequent observation of CO at this R:A atomic ratio. It has become clear that CO in these manganates is closely correlated with size of the A cations [68] which appears to control the Mn-O-Mn bond angle (and notably any deviation from 180o ). This determines the e g bandwidth imposed by the Mn 3d and O 2p hybridization and the hopping process . Therefore, the strength of the double-exchange mechanism is affected. For example, Y 0.5 Ca0.5 MnO3 with the small A cation Y (ca. 1.23Å) not only has the charge-ordering transition temperature (TCO ) in the paramagnetic range, but also the CO is so robust that it is nearly impossible to destroy it by the application of a magnetic field [69]. On the other hand, in the regime of the larger A cations, the ferromagnetic exchange interaction increases, thereby destroying the CO state. In the CO state of R0.5 A0.5 MnO3 a checkerboard arrangement of Mn3+ and Mn4+ occurs. The localized electrons of Mn3+ exhibit orbital degeneracy and develop an OO pattern whereas those in Mn 4+ (t32g ) are nondegenerate. The two possible mechanisms that lead degenerate orbitals to OO is Jahn-Teller distortion and super-exchange interaction [70]. Both the CO and the OO occur simultaneously, with CO as the assumed driving force in most cases [71]. When R and A present in equal amounts, there is a strong competition between the tendency for the orbitals to order locally and the kinetic energy of the charge carriers that tends to destroy long-range order. For the realization of the CO state, EC , Ecf , Eex , and P V (Eq. 7.1) play together simultaneously and the ordered state occurs as a consequence of the joint efforts to minimize the Gibbs energy of the crystalline phase. The different contributors to the Gibbs energy can individually distort the structure or join forces with some or all the others. In the latter case the result can not be regarded as a mere sum of the individual effects but rather as a composite effect produced by an intimate interplay between the different factors. 7.4.1 Types of charge and orbital ordering When charges localize on specific ionic sites in perovskite-like oxides, they take up various patterns of ordering. Only the most-commonly observed ordering patterns are discussed here. In the 50% "doped" manganites, i.e., when Mn occurs in two-different valence states in equal amounts, the most-commonly seen charge ordering is of the checker-boardtype where charges, for example Mn 3+ and Mn4+ , order alternatively [72]. In Fig. 7.3, two different orbital ordering patterns are displayed. Fig. 7.3(a) shows ferro-orbital order where dz 2 orbital of Mn3+ order in phase with each other and the correspondingly empty orbital of Mn4+ . On the other hand in Fig. 7.3(b), dz 2 orbital of Mn3+ stack in an antiferro-(out-ofphase) sequence to give rock-salt arrangement. 86 7.4. CHARGE ORDERING Figure 7.3: Two idealized orbital ordering patterns. (a) Ferro-orbital order and (b) antiferro-orbital order. Blue (seen behind the d z2 orbital) and purple spheres represent Mn3+ and Mn4+ , respectively, in a checker-board-type charge ordered pattern. Figure 7.4: Crystal structure of YBaMn 2 O5 where the two different Mn atoms are shown by different-colored polyhedra. Note the oxygen vacancy in the Y layer, the occupation of which influences the electronic and transport properties of RBaMn2 O5+δ (R = Y and rare-earths). 87 CHAPTER 7. CHARGE AND ORBITAL ORDERING 7.5 Charge and orbital ordering in oxygen-deficient double perovskites Multicomponent perovskite-like oxides such as RBaT 2 O5 (T = transition-metal ions) are promising candidates for versatile functional materials [73]. An ordering at the A site is typically achieved with a systematic distribution of divalent Ba and trivalent R atoms. Oxygen deficiency around the smaller R atoms is a common feature for such phases in which a square-pyramidal coordination is imposed upon the transition metal atoms as a consequence of the layered ordering of R and Ba (formally in 3+ and 2+ states). The atomic arrangement of the resulting structure (Fig. 7.4) has a characteristic appearance which has led to the name double perovskites. The base-plane oxygens of the square pyramids relax toward the R atom. It is the (still formal) R 3+ and Ba2+ charge imbalance in the otherwise delicate structural arrangement which gives rise to oxygen non-stoichiometry expressed as 5+δ in the above formula. With certain rational values for δ typical ordered structure variants occur. For δ = 1/2 also an average half-integer valence state T 2.5+ is established and this can under certain conditions give rise to CO with formal valence states T 3+ and T 2+ . Although a lot of experimental and theoretical attention has been paid on CO and OO in perovskite-like oxides, only a handful of studies have been made on oxygen-deficient double-perovskite oxides. Hence one of the aims of this project has been to analyze CO and OO in YBaT2 O5 and RBaMn2 O5+δ (T = Mn, Fe, and Co; R = Y and La; 0 ≤ δ ≤ 1). The presence of CO and OO in a material is experimentally established by the inferences from superstructure reflections in diffraction measurements, resistivity and heat-capacity measurements, magnetic moment data, structural phase-transition (if any) etc. In our theoretical studies, we earlier made use of the calculated magnetic moments, site-projected DOS and charge-density plots within particular planes to identify the presence of transition-metal atoms in different valence states and visualize their CO features. For example, the presence of T atoms in two different valence states in YBaT 2 O5 with (T = Mn, Fe, and Co) is manifested as the difference in the features of their respective site-projected DOS curves (see Fig. 7.5). Similarly, the orbital-projected DOS provides evidence for the occupation of individual orbitals in the valence band. We used the d-orbital DOS to get insight into the occupancy of individual d orbitals of the T atoms (see for example Fig. 7.6 which shows the DOS of individual d orbitals for Fe in YBaFe2 O5 ). With this approach we could establish the occupation of particular orbitals in the energy-range of interest. In an effort to improve the understanding on ordering phenomena, we later turned to an alternative approach based on the occupation-density matrix of d orbitals within a particular energy interval. With this new tool we are not only able to picture the filling of the orbitals, but also to establish their shape and orientation. The occupation density in the entire valence band, and that from −1 eV to E F enables one to visualize the CO and OO patterns directly. The occupation of the majority-, and minority-spin d levels of Mn in formally 3+ and 2+ states in YBaMn2 O5 are shown as an example in Fig. 7.7(a, b). A clear-cut distinction between the two occupation modes is an indication for the presence of CO on the Mn atoms. Similarly, the d orbital occupancy close 88 7.5. CHARGE AND ORBITAL ORDERING IN OXYGEN-DEFICIENT DOUBLE PEROVSKITES 10 5 Mn1 Mn2 Fe1 Fe2 Co1 Co2 0 −1 atom ) −5 DOS (states eV −1 5 0 −5 5 0 −5 −8 −6 −4 −2 0 2 4 −6 −4 −2 Energy (eV) 0 2 4 6 Figure 7.5: Site-projected density of states (DOS) for the T sites in YBaT 2 O5 (T = Mn, Fe, and Co). to the EF brings about that the dz 2 orbital on Mn3+ is involved whereas the dz 2 and dx2 −y2 orbitals on Mn2+ are seen to form a ferro-orbital-order pattern [Fig. 7.7(c)]. We have used the above-described method to visualize as well as to analyze CO and OO patterns in YBaT2 O5 (as a function of d-orbital filling) and in RBaMn2 O5+δ (as a function of the size of R and Ba as well as oxygen content). The results and the related discussions are elaborately dealt with in Publications I−V. 89 CHAPTER 7. CHARGE AND ORBITAL ORDERING 0.5 Fe1 dz2 Fe2 dz2 0 −0.5 0.5 dx2−y2 dx2−y2 dxy dxy −1 0.5 DOS (states atom eV −0.5 −1 ) 0 0 −0.5 0.5 dxz dxz 0 −0.5 0.5 dyz dyz 0 −0.5 −6 −4 −2 0 2 4 −6 −4 −2 Energy (eV) 0 2 4 6 Figure 7.6: The d-orbital-projected density of states (DOS) for the Fe atoms in YBaFe2 O5 . Figure 7.7: Occupation density of d orbitals of (a) majority-spin, (b) minorityspin bands, and (c) orbital ordering patterns in Mn1 and Mn2 of YBaMn 2 O5 . 90 CHAPTER 8 Summing Up and Looking Ahead ... I seem to have been only like a boy playing on the seashore, and diverting myself now and then finding a smoother pebble or a prettier shell than ordinary, whilst the great ocean of truth lay all undiscovered before me. Sir Issac Newton As I come to the conclusive chapters of this thesis, I sit perplexed and think whether it is an end, or beginning of the end or perhaps the end of a beginning, as Sir Winston Churchil once noted. After nearly four years of research work I feel it may be the beginning of a “beginning”. Among the inorganic materials, transition-metal oxides have acquired special attention owing to the vast diversity of structures and a wide spectrum of exotic properties. We have selected a narrow field, magnetic oxides in complex structures, in particular those consisting of transition-metal atoms in two different valence states. In our attempts to understand such materials, we have perhaps dealt with certain problems for too long or other fascinating problems may have come in between as interludes. Hence our work on the transition-metal oxides have spawned many ideas, some of which have evolved into separate research projects themselves. In fact, some of these are in still in progress while this concluding chapter is being written. In this project we have considered materials such as regular- and distorted-perovskite oxides, regular- and oxygen-deficient double-perovskite oxides, complex one-dimensional oxides, and layered oxides. Even though each of these groups of compounds exhibit greatly differing properties, the common denominator for their selection has been the presence of mixed-valence transition-metal constituents. We have used a number of highly accurate, state-of-the-art tools such as TB-LMTO, VASP, FP-LMTO, FP-LAPW (WIEN2k), and CRYSTAL03, all based on the density-functional theory. The choice of a particular tool has been made depending on the specific problem at hand. During the project period 15 articles have been written among which 8 have been already published in well reputed international journals, 2 accepted for publication and the CHAPTER 8. SUMMING UP AND LOOKING AHEAD remaining contributions are either submitted or included in the thesis in manuscript form. [In addition, I contributed as a co-author in 10 other articles on hydrides, superconducting MgB2 , and multiferroic BiFeO3 (a list of which is given in appendix)]. A major theme of the project has been to understand the intrinsic properties of mixedvalence materials. Hence we have focussed on their ground-state magnetic and electronic properties, bonding behavior, and charge-, and orbital-ordering phenomena. In quite a few cases we have also paid attention on excited-state properties. The main findings of this Dr. Scient. project investigations are listed below. 8.1 Scientific highlights Since the discovery of colossal magneto-resistance extensive works have been performed on manganese oxides. Most of the experimental and theoretical efforts have been devoted to A-site substituted perovskite oxides. Therefore we attempted to study the simultaneous presence of spin, charge, and orbital orderings using the oxygen-deficient double perovskite YBaMn2 O5 as an example. The G-type ferrimagnetic insulating state is found to be the ground state in accordance with experimental findings by using both the full potential LMTO method as well as the full potential LAPW methods. The existence of the two different types of Mn atoms is visualized by differences in site- and orbital-projected DOS curves. The occurrence of checker-board-type charge ordering and ferro-type orbital ordering is established from the charge-density plots. The relatively small size of the Y atoms makes the base-plane Mn-O-Mn bond angle deviate appreciably from 180◦ , which in turn imposes a reduction in the eg band width. The charge- and orbital-ordering features are believed to result from this perturbation of the e g orbitals. We have also calculated the excited-state properties of this material and found that large anisotropy in the optical spectra originates from ferrimagnetic ordering and crystal field splitting. In order to further emphasize the different valence states of Mn, we have calculated K-edge XANE spectra. For Mn as well as O the existence of two types of valence-induced atomic species is established with the help of K-edge spectra (Publication I). Over the years it has been established that hybridization interaction between Mn-d and O-p orbitals have a deciding effect on the electron localization and hence on charge and orbital orderings. Although a lot of attention has been paid to vary the d-electron count by the use of various substituents in perovskite-like solid solution systems, relatively less attention has been paid to variation in the oxygen content. Hence we have carried out model calculations on LaBaMn2 O5+δ (δ = 0, 1/2, 1) and analyzed their ground-state properties in terms of the oxygen content (Publication II). We found that changes in the oxygen content control the valence state of Mn and the hybridization interaction between Mn and O, and consequently varies the double-exchange interactions at the expense of the competing super-exchange interactions. Therefore the electronic ground-state varies from insulator to metal on going from LaBaMn2 O5 to LaBaMn2 O6 , with a reduced band-gap for the interme92 8.1. SCIENTIFIC HIGHLIGHTS diate LaBaMn2 O5.5 phase. In line with this drastic changes in the charge and orbital ordering phenomena have been detected. In an effort to understand the effect of oxygen content as well as the size of R on the charge and orbital ordering, we extended the model calculations to RBaMn 2 O5+δ with R = Y and La (Publication V). There is a somewhat systematic variation in the electronic and magnetic properties with respect to oxygen content in these phases. However the finer features of the ordering schemes such as occupancy of particular orbitals and magnitude of the ordered charges depend largely on the size of R atoms and hence on intricate details of the atomic arrangement. We have also analyzed the changes in ordering features in terms of d-orbital filling by for example, substituting Mn with Fe or Co in YBaMn 2 O5 (Publication IV). We found that the orbital ordering pattern does not change merely with the amount of d electrons available for ordering, but the orbital ordering is more intimately connected with the changes in the structure upon substitution. In short, it is the structural features which determines the ordering of charges and orbitals. We have calculated the electronic and magnetic properties for the quasi-one-dimensional compound Ca3 Co2 O6 for the first time (Publication X). The calculated ferrimagnetic ground state and Co magnetic moments were in good agreement with experimental findings. This compound is interesting since its electronic and magnetic properties appears to be tunable by application of external magnetic fields as well as by electron doping, (substituting Y for Ca). For a particular composition, Ca2 YCo2 O6 we predicted a seldom observed combination of material properties viz. co-existence of ferromagnetism and insulating behaviors. In an initial theoretical study on Ca3 Co2 O6 we concluded with two different valence states for Co which we suggested to correspond to low-spin Co 4+ and to high-spin Co2+ in Publication X. Our work clearly stimulated a lot of subsequent studies, all claiming that the assignment of different valence states for Co in this compound is inappropriate. Hence we have revisited the problem by the use different tools to analyze the valence situation of Co (Publication XI). Our detailed analyses show that neither our critics nor our earlier report brought out the real truth. Our fresh study concluded that the valence of the Co atoms are much smaller than the often believed 3+ state and the valence characteristics are highly directional dependent, in fact about three times more pronounced along the chains than perpendicular to the chains. In the oxygen-deficient perovskite-like oxide Sr 4 Fe4 O11 , the Fe atoms take two different co-ordinations as square pyramids and octahedra. Experimental studies on this compound were able to bring out a magnetic structure with finite magnetic moment at one of the Fe sites and almost zero moment at the other Fe site. In order to better understand this material, we have carried detailed calculations (Publication XV) in which we paid particular 93 CHAPTER 8. SUMMING UP AND LOOKING AHEAD attention to the design of magnetic structure based on the calculated exchange interaction (Jij ) parameter values. Even though we have carried out the calculations using various tools (TBLMTO, FPLMTO, FPLAPW and VASP) all have converged to a solution where both Fe atoms have finite magnetic moments, but with a distinct difference in their values. A deeper analysis shows that, local spin frustration in one of the sites may be the reason for the observation of zero moment by neutron diffraction measurements. Among the several possibilities proposed experimentally, our theoretical results can fit to the model with Fe in square-pyramidal and octahedral environments are in formal oxidation states of 3+ and 4+, respectively. Although spin and orbital dynamics are not unique for manganites, they have received a lot of attention in recent years. In an effort to extend the studies to other mixed-valence transition-metal oxides, we examined for example, systems containing chromates. We have explored structures for a series of compounds ACr 3 O8 (A = H, Li−Cs, In, Tl, Cu, Ag, and Au) which in fact turned out to be one of the most challenging tasks of the entire project. We have predicted ground-state crystal structures for most of these compounds which agree with those established experimentally (Publication VI −IX) where-ever empirical data are available. The calculated equilibrium volumes were found to be over-estimated beyond the limit usually expected for DFT calculations. The overestimation of volume may be attributed to the layered nature of these compounds. Special attention is focussed on the valence state of Cr in these compounds which are believed to possess 3+ and 6+ valence states. However the detailed analysis of their electronic structure shows that Cr 6+ (d0 ) configuration is out of question since none of the Cr have empty d orbitals. Instead the negligible magnetic moment at the Cr site concerned (viz. the Cr atom which has led to assignment Cr6+ ) originates from a negligible exchange splitting. In addition we made a particular study of Cr3 O8 and LiCr3 O8 which have received attention as potential candidates for cathode materials in Li-ion batteries (Publication VII). From the calculated total energy, a new synthesis route is suggested for Cr 3 O8 . The bonding analysis shows that when Li is intercalated into the Cr 3 O8 lattice, Li retains some valence charge and does not donate its valence electron entirely to the Cr 3 O8 framework as usually believed. An orthorhombic perovskite-like oxide SrRuO 3 has a well defined ferromagnetic and metallic ground state. However, for its isostructural counterpart CaRuO 3 there are many controversial reports each claiming a different description of the magnetic state. In an attempt to explore the correct magnetic ground state of CaRuO 3 , we have simulated the magnetic phase diagram for the entire Sr 1−x Cax RuO3 (Publications XII and XIII). In addition to para, and ferromagnetic states we considered A-, C-, and G-type antiferromagnetic configurations. Around the composition x = 0.77 we found a transition from ferromagnetic-toantiferromagnetic state. We also found that CaRuO3 has a G-type antiferromagnetic ground state. However, owing to the very small energy differences between various magnetic con94 8.2. GENERAL INFERENCES figurations, it might have local spin frustration leading to a spin-glass-like behavior. In order to bring out a clearer picture of CaRuO3 , we also carried out an elaborate study on the electronic structure and excited-state properties of this compound. The calculated optical, XPS and Ru-K-edge XANE spectra showed good agreement with available experimental spectra, adding credence to our conclusion on its magnetic ground state. We predicted huge magneto-optical effects for a series of double perovskites A 2 BB O6 (A = Ca, Sr, and Ba; B = Fe; B = Mo, W, and Re). Among these compounds, Sr 2 FeWO6 has the maximum polar Kerr rotation of 3.87◦ and Faraday rotation of 4.5 ×105 deg cm−1 . All the other compounds of this series have both Kerr and Faraday rotation more than 1 ◦ except Ca2 FeMoO6 which has a Kerr rotation of 0.5◦ . It should be recalled that a Kerr rotation value greater than 0.3◦ is considered as technologically significant. The huge magnetooptical effects are found to result from the combined effects of large off-diagonal conductivity, refractive index, magnetic moment, spin-orbit coupling, exchange splitting, band gap, and plasma resonance. Since most of the studied compounds are attractive as potential magneto-resistive materials, our finding on their large magneto-optical effects and ferromagnetic half-metallic nature add further importance to these compounds. 8.2 General Inferences • One of the most important lessons that we learnt from this project is that, valence states can not be approximated as simple formal oxidation states by taking only the ionic character into account. The root of the assignment problem is that part of the atomic arrangement consists of nearly pure ions whereas other parts carry a bonding skeleton of mixed bonding character. For example, the transition metal component is bonded to oxygen by mixed iono-covalent bonds. Therefore, elaborate theoretical studies should be consulted in order to assign valence states in complex systems like those handled in this project. • In some of the earlier publication from this project the oxidation state nomenclature has been used to describe valence state, spin states, and charge ordering. In view of later gained experience such deductions should not be taken too literally until the electronic structure data have been reanalyzed with different tools. • Many experimental oxidation/valence state assignment techniques are based on the use of reference compounds for comparative analysis with compound under investigation. Errors in the oxidation/valence state assignment for the reference substance will then automatically be carried over to the compound under examination. To remedy this defect it is suggested that potential reference substances must be subjected to electronic band structure analysis. • The structural arrangement appears in general to be more decisive for the electronic band 95 BIBLIOGRAPHY structure than the constituents involved. In other words compounds with equal or closely related structural arrangements obtain almost similar DOS. • In order to establish the actual ground-state structure several related structure types were considered as inputs. In order to arrive at the correct structure, the input test structures should reasonably describe the actual atomic arrangement. Even if the test the structure does not provide all the symmetry constraints, it should be reasonably close to the real situation. This implies that the selection of proper of test input structures will simplify the structural optimization procedure. • From the structural optimization of a couple of close packed compounds we found that the overestimation of calculated volume compared to the experimental volume is well within the limits of DFT calculations. On the other hand, the overestimation of volume is above commonly accepted limits for a series of layered compounds. Therefore, in order to estimate cohesive properties of layered compounds where van der Waals forces are more dominant, usual DFT calculations are not sufficient. • The experimentally observed insulating/semiconducting behavior can only be computationally simulated when the experimentally observed co-operative magnetic arrangement is introduced into the input model. • From the overall analysis one can note that the use of usual LDA and GGA were able to reproduce and explain most of the experimental findings for the compounds dealt in this project. Therefore correlation effects are not as strong in the compounds studied here as commonly believed. Therefore additional approximations such as LDA+U methods are seldom needed to explain their behavior. 8.3 Next step As we already mentioned during the course of this project several sub-projects cropped up and also new problems have evolved. In future we plan to extend the study on spin, charge, and orbital orderings to YBaT 2 O5+δ (T = Co and Fe; δ = 1/2 and 1). An experimental measurement of XPS on Ca3 Co2 O6 has suggested 3+ valence states for Co constituents. Therefore we plan to simulate the XPS profile for this compound in order to evaluate the experimental claim. Moreover, for the double perovskites A 2 FeBO6 (A = Ca, Sr, Ba; B = Mo, W, Re) half-metallic electronic structure is observed only in the ferromagnetic configuration whereas for some of these compounds ferrimagnetic configurations is proposed. So a planned extension of the present work is to carry out extensive studies on electronic and magnetic properties of the A 2 FeBO6 series. In the present calculations, only collinear magnetic configurations have been considered. However, non-collinear magnetic arrangements should be properly taken care of in contin96 BIBLIOGRAPHY ued projects. For the calculation of excited-state properties, excitonic effects should also be included together with improvements like GW approximations. Finally, better tools should be devised for evaluation of the real valence states of components. 97 BIBLIOGRAPHY 98 BIBLIOGRAPHY [1] C.S. Smith. On material structure and human history. Annu. Rev. Mater. Sci., 16:1, (1986). [2] H. Hohenberg and W. Kohn. Phys. Rev., 136:864, (1964). [3] M.T. Yin and M.L. Cohen. Phys. Rev. B, 51:13987, (1982). [4] J. Neugebauer and M. Scheffler. Phys. Rev. B, 46:16067, (1992). [5] J.L. Simonds. Physics Today, 48:26, 1995. [6] K.G. Wilson. Rev. Mod. Phys., 47(4):773, (1975). [7] N.W. Ashcroft and N.D. Mermin. Solid State Physics. (Saunders College Printing, USA, 1976). [8] W. Kohn. Rev. Mod. Phys., 71:1253, (1998). [9] W. Kohn and L.J. Sham. PRA, 140:1133, 1965. [10] R.O. Jones and O. Gunnarsson. Rev. Mod. Phys., 61:689, (1989). [11] D.J. Singh. Planewaves, Psuedopotentials, and the LAPW method. (Kluwer, USA, 1994). [12] J.P. Perdew and Y. Wang. Phys. Rev. B, 45:13244, (1992). [13] J.P. Perdew, K. Burke, and M. Ernerhof. Phys. Rev. Lett., 82:2544, (1996). [14] H.L. Skriver. The LMTO Method. (Springer, 1984, 1984). [15] M. Methfessel. Phys. Rev. B, 38:1537, (1988). [16] O.K. Andersen. Computational Methods in Band Theory. (Plenum, New York, 1971). 99 BIBLIOGRAPHY [17] R.M. Martin. Electronic Structure: Basic Theory and Practical Methods. (Cambridge University Press, 2004). [18] A. Burkhardt G. krier, O. Jepsen. Tight Binding LMTO-ASA Program, Version 4.7. (O. K. Andersen, Stuttgart, Germany, 1999). [19] J.M. Wills, O. Eriksson, and M. Alouani. in "Electronic Structure and Physical Properties of Solids", ed. by H. Dressey. (Springer Verlag, Berlin, 2000). [20] J. Trygg. First Principles Studies of Magnetic and Structural Properties of Metallic Systems. (PhD Thesis, Uppsala University, 1995). [21] P. Blaha, K. Schwarz, and J. Luitz. A Full Potential Linearized Augmented Planewave Package for Calculating Crystal Properties. (Technical University Wien, Vienna, ISBN 39501031-0-4, 2003). [22] M. Weinert, E. Wimmer, and A. J. Freeman. Phys. Rev. B, 26:4571, (1982). [23] N.A. Spaldin and W.E. Pickett. J. Solid State Chem., 176:615, (2003). [24] M.L. Cohen. Annu. Rev. Mater. Sci., 30:1, (2000). [25] P.E. Blöchl. Phys. Rev. B, 50:17953, (1994). [26] G. Kresse and J. Hafner. Phys. Rev. B, 47:R6726, (1993). [27] G. Kresse and D. Joubert. Phys. Rev. B, 59:1758, (1999). [28] F.D. Murnaghan. Proc. Natl. Acad. Sci., 30:8244, (1944). [29] F. Birch. Phys. Rev., 71:809, (1947). [30] F. Birch. J. Geophys. Res., 83:1257, (1978). [31] P. Vinet, J. Ferrante, J.R. Smith, and J.H. Rose. J. Phys. C, 19:467, (1986). [32] C.D. Gelatt.Jr., A.R. Williams, and V.L. Moruzzi. Phys. Rev. B, 27:2005, (1983). [33] R. Dronskowski and P.E. Blöchl. J. Phys. Chem., 97:8617, (1993). [34] P. Blaha J.M. Zuo and K. Schwarz. J. Phys.: Condens. Matter, 9:7541, (1997). [35] B. Silvi and A. Savin. Nature, 371:683, (1994). [36] A. Savin, A.D. Becke, J. Flad, R. Nesper, H. Preuss, and H.G. von Schnerring. Angew. Chem. Int. Ed. Engl., 30:409, (1991). [37] A.D. Becke and K.E. Edgecombe. J. Chem. Phys., 92:5397, (1990). 100 BIBLIOGRAPHY [38] R.F.W. Bader. Atoms in Molecules: A Quantum Theory. (Clarendon Press, Oxford, 1990). [39] R.M. Martin. Phys. Rev. B, 9:1998, (1974). [40] M.H. Cohen R. Pick and R.M. Martin. Phys. Rev. B, 1:910, (1970). [41] A. Görling. Phys. Rev. A, 54:3912, (1996). [42] F. Wooten. Optical Properties of Solids. (Academic, New York, 1972). [43] R. Kubo. J. Phys. Soc. Jpn., 12:570, (1957). [44] C.S. Wang and J. Callaway. Phys. Rev. B, 9:4897, (1974). [45] M. Born. Principles of Optics. (Springer, London, 1964). [46] J. Kerr. Phil. Mag., 3:321, (1877). [47] M. Faraday. Phil. Trans. Roy. Soc., 136:1, (1846). [48] F.J. Kahn, P.S. Pershan, and J.P. Remeika. Phys. Rev., 186:891, (1969). [49] W. Reim, J. Schoenes, Eds. K.H.K. Buschow, and E.P. Wohlfarth. Ferromagnetic Materials, 5(Chap. 2), (1990). [50] P.G. van Engen, K.H.J. Buschow, R. Jongebreur, and M. Erman. Appl. Phys. Lett., 42:202, (1983). [51] P.J. Grundy. Electronic and magnetic properties of metals and ceramics. Materials Science and Technology, 3B, (1994). [52] M. Mansuripur. The Physical Principles of Magneto-optical Recording. (Cambridge University Press, Cambridge, 1995). [53] A. Neckel, K. Schwarz, R. Eibler, and P. Rastl. Microchim. Acta Suppl., 6:257, (1975). [54] C. Kittel. Introduction to Solid State Physics. (Wiley, New York, 1971). [55] U. Müller. Inorganic Structural Chemistry. (Wiley, Chichester, 1993). [56] C. Zener. Phys. Rev., 82:402, (1951). [57] P.W. Anderson and H. Hasegawa. Phys. Rev., 100:675, (1955). [58] Y. Tokura and N. Nagaosa. Science, 288:462, (2000). [59] J.M.D. Coey, M. Viret, and S. von Molnár. Adv. Phys., 48:167, (1999). [60] A.R. West. Solid State Chemistry and its Applications. (Wiley, Chichester, 1984). 101 BIBLIOGRAPHY [61] E. Pollert. Int. J. Inorg. Mater., 2:661, (2000). [62] M.B. Robin and P. Day. Adv. Inorg. Chem. Radiochem., 10:247, (1967). [63] C.N.R. Rao and A.K. Cheetham. Science, 272:369, (1996). [64] H.A. Jahn and E. Teller. Proc. R. Soc. London, 220:A161, (1937). [65] J.B. Goodenough. Magnetism and the Chemical Bond. (Interscience, New York, 1963). [66] C.N.R. Rao, A. Arulraj, A.K. Cheetham, and B. Raveau. J.Phys.: Condens. Matter., 12:R83, (2000). [67] E.J.W. Verwey. Nature (London), 144:327, (1939). [68] C.N.R. Rao and A.K. Cheetham. Science, 276:911, (1997). [69] C.N.R. Rao and P.V. Vanitha. Curr. Opinion Solid State Mater. Sci., 6:97, (2002). [70] J. van den Brink, G. Khaliullin, D. Khomskii, and Ed.T. Chatterji. Colossal Magnetoresistive Manganites. (Springer, 2002). [71] D. Khomskii and G. Sawastzky. Solid State Commun., 102:87, (1997). [72] A.J. Williams and J.P. Attfield. Phys. Rev. B, 72:024436, (2005). [73] P.M. Woodward and P. Karen. Inorg. Chem., 42:1121, (2003). 102 List of Publications 103 List of Publications 104 List of publications The way of progress is neither swift nor easy. Marie Curie I. Spin, charge and orbital ordering in the ferrimagnetic insulator YBaMn2 O5 R.Vidya, P. Ravindran, A. Kjekshus, and H. Fjellvåg Phys. Rev. B. 65, 144422 (2002). II. Effect of oxygen stoichiometry on spin, charge, and orbital ordering in manganites R. Vidya, P. Ravindran, P. Vajeeston, A. Kjekshus, and H. Fjellvåg Phys. Rev. B 69, 092405 (2004). III. Spin, charge, and orbital ordering in oxides with dual-valent transition-metal ions R. Vidya, P. Ravindran, P. Vajeeston, H. Fjellvåg and A. Kjekshus Ceramics International 30, 1993 (2004). IV. Effect of d-band filling on spin, charge and orbital ordering in YBaT2 O5 (T = Mn, Fe, Co) R. Vidya, P. Ravindran, K. Knizek, A. Kjekshus, and H. Fjellvåg In manuscript. V. Spin, charge, and orbital ordering in RBaMn2 O5+δ (R = Y, La; 0 ≤ δ ≤ 1) and their dependence on oxygen content and size of R constituent R. Vidya, P. Ravindran, A. Kjekshus, and H. Fjellvåg In manuscript. VI. Structural stability, electronic structure and magnetic properties of mixed-valence ACr3 O8 phases (A = Na, K, and Rb) R. Vidya, P. Ravindran, P. Vajeeston, H. Fjellvåg, and A. Kjekshus Phys. Rev. B 72, 014411 (2005). List of Publications VII. Crystal and electronic structures of Cr3 O8 and LiCr3 O8 : Probable cathode materials in Li batteries R. Vidya, P. Ravindran, H. Fjellvåg, and A. Kjekshus Phys. Rev. B (accepted). VIII. Density-functional calculations of crystal structures and properties of CsCr3 O8 and ACr3 O8 (A = In, Tl, Cu, Ag, Au) R. Vidya, P. Ravindran, H. Fjellvåg, and A. Kjekshus Submitted to Phys. Rev. B IX. First-principles density-functional calculations on HCr3 O8 : An exercise to better understand the ACr3 O8 (A = alkali-metal) family R. Vidya, P. Ravindran, H. Fjellvåg, and A. Kjekshus J. Electrochem. Soc. (accepted). X. Tailor-made electronic and magnetic properties in one-dimensional pure and Ysubstituted Ca3 Co2 O6 R. Vidya, P. Ravindran , H. Fjellvåg, A. Kjekshus, and O. Eriksson Phys. Rev. Lett. 91, 186404 (2003). XI. Valence states and associated features of Co in quasi-one-dimensional Ca3 Co2 O6 R. Vidya, P. Ravindran, H. Fjellvåg, and A. Kjekshus In manuscript. XII. Antiferromagnetic vs. ferromagnetic interactions and spin-glass-like behavior in ruthenates P. Ravindran, R. Vidya, P. Vajeeston, A. Kjekshus, H. Fjellvåg, and B.C. Hauback Solid State Commun. 124, 293 (2002). XIII. Magnetic properties of Ca-doped SrRuO3 from full-potential calculations R. Vidya, P. Ravindran, A. Kjekshus, H. Fjellvåg, and B.C. Hauback J. Solid State Chem. 177, 146 (2004). XIV. Huge magneto-optical effects in half-metallic double perovskites R. Vidya, P. Ravindran, A. Kjekshus, and H. Fjellvåg Phys. Rev. B 70, 184414 (2004). XV. Spin- and charge-ordering in oxygen-vacancy-ordered mixed-valence Sr4 Fe4 O11 R. Vidya, P. Ravindran, A. Kjekshus, and H. Fjellvåg In manuscript. 106 Appendix Publications not included in this thesis I. Origin of multiferroic behavior in BiFeO3 P. Ravindran, R. Vidya, A. Klaveness, F. Tylholdt, H. Fjellvåg, and A. Kjekshus Submitted to Phys. Rev. B II. Indicator for site preference of hydrogen in metals, alloys, and intermetallic frameworks P. Vajeeston, P. Ravindran, R. Vidya, H. Fjellvåg, and A. Kjekshus Euro. Phys. Lett. 72, 569 (2005). III. Ground state and excited state properties of inorganic solids from full-potential density functional calculations P. Ravindran, R. Vidya, P. Vajeeston, A. Kjekshus and H. Fjellvåg J. Solid State Chemistry (review) 176, 338-374 (2003). IV. Design of Potential Hydrogen-storage Material using First-principle Densityfunctional Calculations P. Vajeeston, P. Ravindran , R. Vidya, H. Fjellvåg, and A. Kjekshus Cry. Growth & Design 4, 471-477 (2004). V. Electronic Structure and Excited-state Properties of Perovskite-like Oxides P. Ravindran, R. Vidya, A. Kjekshus and H. Fjellvåg J. Cryst. Growth 268, 554-559 (2004). 107 List of Publications VI. VII. VIII. A pressure-induced phase of NaAlH4 : A potential candidate for hydrogen storage? P. Vajeeston, P. Ravindran, R. Vidya, H. Fjellvåg, and A. Kjekshus Appl. Phys. Lett. 82, 2257 (2003). Short hydrogen-hydrogen separation in RNiInH 1.333 (R=La, Ce, Nd) P. Vajeeston, P. Ravindran, R. Vidya, A. Kjekshus, H. Fjellvåg and V.A. Yartys Phys. Rev. B 67, 014101 (2003). Violation of the “2 Å rule" for Metal Hydrides P. Ravindran, P. Vajeeston, R. Vidya, A. Kjekshus and H. Fjellvåg Phys. Rev. Lett. 89, 106403 (2002). IX. Electronic structure, phase stability and chemical bonding in Th2 Al and Th2 AlH4 P. Vajeeston, R. Vidya, P. Ravindran, H. Fjellvåg, A. Kjekshus and A. Skjeltorp Phys. Rev. B 65, 075101 (2002). X. Detailed electronic structure studies on superconducting MgB2 and related compounds P. Ravindran, P. Vajeeston, R. Vidya, A. Kjekshus and H. Fjellvåg Phys. Rev. B. 64, 224509(1-15) (2001). 108